#------------------------------------------------------------------------------
#$Date: 2016-03-22 23:45:32 +0200 (Tue, 22 Mar 2016) $
#$Revision: 179076 $
#$URL: svn://www.crystallography.net/cod/cif/4/30/38/4303828.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4303828
loop_
_publ_author_name
'Pavlo Solokha'
'Serena De Negri'
'Volodymyr Pavlyuk'
'Adriana Saccone'
_publ_section_title
;
Anti-Mackay Polyicosahedral Clusters in La-Ni-Mg Ternary Compounds:
Synthesis and Crystal Structure of the La43Ni17Mg5 New Intermetallic Phase
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              11586
_journal_page_last               11593
_journal_paper_doi               10.1021/ic901422v
_journal_volume                  48
_journal_year                    2009
_chemical_formula_moiety         'La43 Ni17, 5(Mg)'
_chemical_formula_sum            'La43 Mg5 Ni17'
_chemical_formula_weight         7092.75
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           63
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-C 2c 2'
_symmetry_space_group_name_H-M   'C m c m'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   10.1895(3)
_cell_length_b                   17.6044(14)
_cell_length_c                   42.170(3)
_cell_measurement_reflns_used    3384
_cell_measurement_temperature    295(2)
_cell_measurement_theta_max      26.37
_cell_measurement_theta_min      2.31
_cell_volume                     7564.5(8)
_computing_cell_refinement       'CrysAlis CCD (Oxford Diffraction, 2004)'
_computing_data_collection       'CrysAlis CCD (Oxford Diffraction, 2004)'
_computing_data_reduction        'CrysAlis RED (Oxford Diffraction, 2005)'
_computing_publication_material  'SHELX-97 (Sheldrick, 1997)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1997)'
_diffrn_ambient_temperature      295(2)
_diffrn_detector_area_resol_mean 0
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'Xcalibur Oxford Diffraction'
_diffrn_measurement_method       'ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0528
_diffrn_reflns_av_sigmaI/netI    0.0414
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       22
_diffrn_reflns_limit_k_min       -21
_diffrn_reflns_limit_l_max       47
_diffrn_reflns_limit_l_min       -52
_diffrn_reflns_number            24183
_diffrn_reflns_theta_full        26.37
_diffrn_reflns_theta_max         26.37
_diffrn_reflns_theta_min         2.31
_diffrn_standards_decay_%        0
_diffrn_standards_interval_count 0
_diffrn_standards_interval_time  0
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    27.799
_exptl_absorpt_correction_T_max  0.122
_exptl_absorpt_correction_T_min  0.031
_exptl_absorpt_correction_type   analytical
_exptl_absorpt_process_details   'CrysAlis RED (Oxford Diffraction, 2005)'
_exptl_crystal_colour            'metal grey'
_exptl_crystal_density_diffrn    6.228
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       'irregularly shaped'
_exptl_crystal_F_000             11948
_exptl_crystal_size_max          0.48
_exptl_crystal_size_mid          0.12
_exptl_crystal_size_min          0.08
_refine_diff_density_max         6.739
_refine_diff_density_min         -3.432
_refine_diff_density_rms         0.425
_refine_ls_extinction_coef       0.0000117(15)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.179
_refine_ls_matrix_type           full
_refine_ls_number_parameters     176
_refine_ls_number_reflns         4157
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.179
_refine_ls_R_factor_all          0.0840
_refine_ls_R_factor_gt           0.0598
_refine_ls_shift/su_max          0.052
_refine_ls_shift/su_mean         0.002
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0251P)²+563.4628P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0897
_refine_ls_wR_factor_ref         0.0962
_reflns_number_gt                3384
_reflns_number_total             4157
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic901422v_si_001.cif
_cod_data_source_block           mnl70
_cod_depositor_comments
;
The following automatic conversions were performed:
'_symmetry_cell_setting' value 'Orthorhombic' changed to 'orthorhombic'
according to '/home/saulius/struct/CIF-dictionaries/cif_core.dic'
dictionary named 'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_enum 1527 2010-12-29 10:47:43Z saulius 
;
_cod_database_code               4303828
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z+1/2'
'-x, y, -z+1/2'
'x, -y, -z'
'x+1/2, y+1/2, z'
'-x+1/2, -y+1/2, z+1/2'
'-x+1/2, y+1/2, -z+1/2'
'x+1/2, -y+1/2, -z'
'-x, -y, -z'
'x, y, -z-1/2'
'x, -y, z-1/2'
'-x, y, z'
'-x+1/2, -y+1/2, -z'
'x+1/2, y+1/2, -z-1/2'
'x+1/2, -y+1/2, z-1/2'
'-x+1/2, y+1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
La1 La 0.0000 0.38998(11) 0.2500 0.0153(4) Uani 1 4 d S . .
La2 La 0.18607(13) 0.20422(8) 0.2500 0.0152(3) Uani 1 2 d S . .
La3 La 0.0000 0.13923(8) 0.17412(3) 0.0144(3) Uani 1 2 d S . .
La4 La 0.18828(9) 0.32898(5) 0.17400(2) 0.0141(2) Uani 1 1 d . . .
La5 La 0.0000 0.72780(7) 0.20648(3) 0.0129(3) Uani 1 2 d S . .
La6 La 0.0000 0.19723(8) 0.62632(3) 0.0142(3) Uani 1 2 d S . .
La7 La 0.19344(9) 0.20140(5) 0.10123(2) 0.0139(2) Uani 1 1 d . . .
La8 La 0.30731(9) 0.03499(5) 0.20655(2) 0.0131(2) Uani 1 1 d . . .
La9 La 0.30495(9) 0.49596(5) 0.12681(2) 0.0142(2) Uani 1 1 d . . .
La10 La 0.19578(9) 0.33018(5) 0.02600(2) 0.0146(2) Uani 1 1 d . . .
La11 La 0.0000 0.13880(8) 0.02884(3) 0.0130(3) Uani 1 2 d S . .
La12 La 0.0000 0.39065(8) 0.09880(3) 0.0139(3) Uani 1 2 d S . .
La13 La 0.0000 0.06788(8) 0.55569(3) 0.0120(3) Uani 1 2 d S . .
La14 La 0.0000 0.59876(8) 0.13280(3) 0.0145(3) Uani 1 2 d S . .
La15 La 0.0000 0.28079(9) 0.54761(4) 0.0219(3) Uani 1 2 d S . .
La16 La 0.31697(9) 0.03483(5) 0.04522(2) 0.0144(2) Uani 1 1 d . . .
Ni1 Ni 0.0000 0.07797(17) 0.09224(8) 0.0182(7) Uani 1 2 d S . .
Ni2 Ni 0.0000 0.45337(17) 0.16750(8) 0.0184(7) Uani 1 2 d S . .
Ni3 Ni 0.2812(2) 0.17213(12) 0.16828(5) 0.0170(5) Uani 1 1 d . . .
Ni4 Ni 0.2807(2) 0.35936(13) 0.09067(5) 0.0183(5) Uani 1 1 d . . .
Ni5 Ni 0.0000 0.5987(3) 0.2500 0.0164(9) Uani 1 4 d S . .
Ni6 Ni 0.0000 0.43146(19) 0.00910(8) 0.0212(7) Uani 1 2 d S . .
Ni7 Ni 0.1275(3) 0.0000 0.0000 0.0234(7) Uani 1 2 d S . .
Mg1 Mg 0.3338(10) 0.3774(5) 0.2500 0.027(2) Uani 1 2 d S . .
Mg2 Mg 0.0000 0.0678(5) 0.6912(3) 0.029(2) Uani 1 2 d S . .
Mg3 Mg 0.0000 0.0432(8) 0.2500 0.026(3) Uani 1 4 d S . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
La La -0.2871 2.4523 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mg Mg 0.0486 0.0363 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ni Ni 0.3393 1.1124 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
Mg1 La1 Mg1 172.6(3) . 3 ?
Mg1 La1 La8 61.05(12) . 7 ?
Mg1 La1 La8 124.99(13) 3 7 ?
Mg1 La1 La8 61.05(12) . 16 ?
Mg1 La1 La8 124.99(12) 3 16 ?
La8 La1 La8 59.28(4) 7 16 ?
Mg1 La1 La8 124.99(12) . 14_456 ?
Mg1 La1 La8 61.05(12) 3 14_456 ?
La8 La1 La8 64.00(4) 7 14_456 ?
La8 La1 La8 92.90(5) 16 14_456 ?
Mg1 La1 La8 124.99(12) . 5_455 ?
Mg1 La1 La8 61.05(12) 3 5_455 ?
La8 La1 La8 92.90(5) 7 5_455 ?
La8 La1 La8 64.00(4) 16 5_455 ?
La8 La1 La8 59.28(4) 14_456 5_455 ?
Mg1 La1 La2 116.39(16) . 3 ?
Mg1 La1 La2 56.18(15) 3 3 ?
La8 La1 La2 149.52(2) 7 3 ?
La8 La1 La2 149.52(2) 16 3 ?
La8 La1 La2 109.28(2) 14_456 3 ?
La8 La1 La2 109.28(2) 5_455 3 ?
Mg1 La1 La2 56.18(15) . . ?
Mg1 La1 La2 116.39(16) 3 . ?
La8 La1 La2 109.28(2) 7 . ?
La8 La1 La2 109.28(2) 16 . ?
La8 La1 La2 149.52(2) 14_456 . ?
La8 La1 La2 149.52(2) 5_455 . ?
La2 La1 La2 60.21(5) 3 . ?
Mg1 La1 La4 118.34(6) . 12 ?
Mg1 La1 La4 59.30(4) 3 12 ?
La8 La1 La4 149.29(5) 7 12 ?
La8 La1 La4 92.53(2) 16 12 ?
La8 La1 La4 109.67(3) 14_456 12 ?
La8 La1 La4 61.38(2) 5_455 12 ?
La2 La1 La4 60.88(2) 3 12 ?
La2 La1 La4 90.49(4) . 12 ?
Mg1 La1 La4 59.30(4) . . ?
Mg1 La1 La4 118.34(6) 3 . ?
La8 La1 La4 109.67(3) 7 . ?
La8 La1 La4 61.38(2) 16 . ?
La8 La1 La4 149.29(5) 14_456 . ?
La8 La1 La4 92.53(2) 5_455 . ?
La2 La1 La4 90.49(4) 3 . ?
La2 La1 La4 60.88(2) . . ?
La4 La1 La4 59.16(3) 12 . ?
Mg1 La1 La4 59.30(4) . 10_556 ?
Mg1 La1 La4 118.34(6) 3 10_556 ?
La8 La1 La4 61.38(2) 7 10_556 ?
La8 La1 La4 109.67(3) 16 10_556 ?
La8 La1 La4 92.53(2) 14_456 10_556 ?
La8 La1 La4 149.29(5) 5_455 10_556 ?
La2 La1 La4 90.49(4) 3 10_556 ?
La2 La1 La4 60.88(2) . 10_556 ?
La4 La1 La4 147.92(6) 12 10_556 ?
La4 La1 La4 111.10(4) . 10_556 ?
Mg1 La1 La4 118.34(6) . 3 ?
Mg1 La1 La4 59.30(4) 3 3 ?
La8 La1 La4 92.53(2) 7 3 ?
La8 La1 La4 149.29(5) 16 3 ?
La8 La1 La4 61.38(2) 14_456 3 ?
La8 La1 La4 109.67(3) 5_455 3 ?
La2 La1 La4 60.88(2) 3 3 ?
La2 La1 La4 90.49(4) . 3 ?
La4 La1 La4 111.10(4) 12 3 ?
La4 La1 La4 147.92(6) . 3 ?
La4 La1 La4 59.16(3) 10_556 3 ?
Mg1 La2 Mg3 172.5(2) . . ?
Mg1 La2 La8 124.94(12) . . ?
Mg3 La2 La8 61.16(12) . . ?
Mg1 La2 La8 124.94(12) . 10_556 ?
Mg3 La2 La8 61.16(12) . 10_556 ?
La8 La2 La8 59.21(3) . 10_556 ?
Mg1 La2 La5 61.19(13) . 14_546 ?
Mg3 La2 La5 124.90(12) . 14_546 ?
La8 La2 La5 92.70(4) . 14_546 ?
La8 La2 La5 63.80(3) 10_556 14_546 ?
Mg1 La2 La5 61.19(13) . 5_545 ?
Mg3 La2 La5 124.90(12) . 5_545 ?
La8 La2 La5 63.80(3) . 5_545 ?
La8 La2 La5 92.70(4) 10_556 5_545 ?
La5 La2 La5 59.28(4) 14_546 5_545 ?
Mg1 La2 La1 56.38(15) . . ?
Mg3 La2 La1 116.12(15) . . ?
La8 La2 La1 149.53(2) . . ?
La8 La2 La1 149.53(2) 10_556 . ?
La5 La2 La1 109.61(4) 14_546 . ?
La5 La2 La1 109.61(4) 5_545 . ?
Mg1 La2 La2 116.28(15) . 3 ?
Mg3 La2 La2 56.22(14) . 3 ?
La8 La2 La2 109.45(3) . 3 ?
La8 La2 La2 109.45(3) 10_556 3 ?
La5 La2 La2 149.53(2) 14_546 3 ?
La5 La2 La2 149.53(2) 5_545 3 ?
La1 La2 La2 59.90(3) . 3 ?
Mg1 La2 La4 59.37(5) . 10_556 ?
Mg3 La2 La4 118.24(6) . 10_556 ?
La8 La2 La4 149.27(4) . 10_556 ?
La8 La2 La4 92.56(2) 10_556 10_556 ?
La5 La2 La4 61.57(3) 14_546 10_556 ?
La5 La2 La4 109.86(4) 5_545 10_556 ?
La1 La2 La4 60.91(2) . 10_556 ?
La2 La2 La4 90.33(3) 3 10_556 ?
Mg1 La2 La4 59.37(5) . . ?
Mg3 La2 La4 118.24(6) . . ?
La8 La2 La4 92.56(2) . . ?
La8 La2 La4 149.27(4) 10_556 . ?
La5 La2 La4 109.86(4) 14_546 . ?
La5 La2 La4 61.57(3) 5_545 . ?
La1 La2 La4 60.91(2) . . ?
La2 La2 La4 90.33(3) 3 . ?
La4 La2 La4 111.15(4) 10_556 . ?
Mg1 La2 La3 118.64(6) . . ?
Mg3 La2 La3 58.99(5) . . ?
La8 La2 La3 61.31(2) . . ?
La8 La2 La3 109.41(4) 10_556 . ?
La5 La2 La3 149.26(4) 14_546 . ?
La5 La2 La3 92.65(2) 5_545 . ?
La1 La2 La3 90.57(3) . . ?
La2 La2 La3 60.84(2) 3 . ?
La4 La2 La3 147.92(4) 10_556 . ?
La4 La2 La3 59.38(3) . . ?
Mg1 La2 La3 118.64(6) . 10_556 ?
Mg3 La2 La3 58.99(5) . 10_556 ?
La8 La2 La3 109.41(4) . 10_556 ?
La8 La2 La3 61.31(2) 10_556 10_556 ?
La5 La2 La3 92.65(2) 14_546 10_556 ?
La5 La2 La3 149.26(4) 5_545 10_556 ?
La1 La2 La3 90.57(3) . 10_556 ?
La2 La2 La3 60.84(2) 3 10_556 ?
La4 La2 La3 59.38(3) 10_556 10_556 ?
La4 La2 La3 147.92(4) . 10_556 ?
La3 La2 La3 110.63(4) . 10_556 ?
Ni3 La3 Ni3 155.23(10) 12 . ?
Ni3 La3 Ni1 88.79(5) 12 . ?
Ni3 La3 Ni1 88.79(5) . . ?
Ni3 La3 Mg3 99.58(6) 12 . ?
Ni3 La3 Mg3 99.58(6) . . ?
Ni1 La3 Mg3 134.8(2) . . ?
Ni3 La3 Mg2 102.12(5) 12 2_554 ?
Ni3 La3 Mg2 102.12(5) . 2_554 ?
Ni1 La3 Mg2 83.80(18) . 2_554 ?
Mg3 La3 Mg2 51.0(3) . 2_554 ?
Ni3 La3 La9 64.79(5) 12 5_445 ?
Ni3 La3 La9 126.94(6) . 5_445 ?
Ni1 La3 La9 45.36(4) . 5_445 ?
Mg3 La3 La9 98.92(18) . 5_445 ?
Mg2 La3 La9 56.46(13) 2_554 5_445 ?
Ni3 La3 La9 126.94(6) 12 16_545 ?
Ni3 La3 La9 64.79(5) . 16_545 ?
Ni1 La3 La9 45.36(4) . 16_545 ?
Mg3 La3 La9 98.92(18) . 16_545 ?
Mg2 La3 La9 56.46(13) 2_554 16_545 ?
La9 La3 La9 63.43(4) 5_445 16_545 ?
Ni3 La3 La7 51.00(5) 12 12 ?
Ni3 La3 La7 112.38(6) . 12 ?
Ni1 La3 La7 46.84(4) . 12 ?
Mg3 La3 La7 147.89(5) . 12 ?
Mg2 La3 La7 115.95(14) 2_554 12 ?
La9 La3 La7 59.61(3) 5_445 12 ?
La9 La3 La7 92.17(3) 16_545 12 ?
Ni3 La3 La7 112.38(6) 12 . ?
Ni3 La3 La7 51.00(5) . . ?
Ni1 La3 La7 46.84(4) . . ?
Mg3 La3 La7 147.89(5) . . ?
Mg2 La3 La7 115.95(14) 2_554 . ?
La9 La3 La7 92.17(3) 5_445 . ?
La9 La3 La7 59.61(3) 16_545 . ?
La7 La3 La7 62.28(4) 12 . ?
Ni3 La3 La4 108.37(6) 12 . ?
Ni3 La3 La4 48.87(5) . . ?
Ni1 La3 La4 104.92(5) . . ?
Mg3 La3 La4 113.96(18) . . ?
Mg2 La3 La4 148.32(6) 2_554 . ?
La9 La3 La4 147.11(4) 5_445 . ?
La9 La3 La4 108.43(3) 16_545 . ?
La7 La3 La4 90.43(3) 12 . ?
La7 La3 La4 59.50(3) . . ?
Ni3 La3 La4 48.87(5) 12 12 ?
Ni3 La3 La4 108.37(6) . 12 ?
Ni1 La3 La4 104.92(5) . 12 ?
Mg3 La3 La4 113.96(18) . 12 ?
Mg2 La3 La4 148.32(6) 2_554 12 ?
La9 La3 La4 108.43(3) 5_445 12 ?
La9 La3 La4 147.11(4) 16_545 12 ?
La7 La3 La4 59.50(3) 12 12 ?
La7 La3 La4 90.43(3) . 12 ?
La4 La3 La4 59.74(4) . 12 ?
Ni3 La3 La8 48.27(4) 12 12 ?
Ni3 La3 La8 155.72(6) . 12 ?
Ni1 La3 La8 101.27(4) . 12 ?
Mg3 La3 La8 57.81(7) . 12 ?
Mg2 La3 La8 57.83(6) 2_554 12 ?
La9 La3 La8 56.36(2) 5_445 12 ?
La9 La3 La8 107.15(4) 16_545 12 ?
La7 La3 La8 90.15(2) 12 12 ?
La7 La3 La8 146.89(4) . 12 ?
La4 La3 La8 144.37(4) . 12 ?
La4 La3 La8 90.50(2) 12 12 ?
Ni2 La4 Ni3 155.54(7) . . ?
Ni2 La4 Mg1 100.06(14) . . ?
Ni3 La4 Mg1 99.33(14) . . ?
Ni2 La4 Mg2 102.25(12) . 6_554 ?
Ni3 La4 Mg2 101.53(12) . 6_554 ?
Mg1 La4 Mg2 50.7(2) . 6_554 ?
Ni2 La4 La9 64.56(5) . . ?
Ni3 La4 La9 126.43(5) . . ?
Mg1 La4 La9 98.92(14) . . ?
Mg2 La4 La9 56.65(15) 6_554 . ?
Ni2 La4 La6 126.27(6) . 6_554 ?
Ni3 La4 La6 64.56(5) . 6_554 ?
Mg1 La4 La6 98.90(14) . 6_554 ?
Mg2 La4 La6 56.50(15) 6_554 6_554 ?
La9 La4 La6 63.07(3) . 6_554 ?
Ni2 La4 La7 112.06(7) . . ?
Ni3 La4 La7 51.12(5) . . ?
Mg1 La4 La7 147.65(13) . . ?
Mg2 La4 La7 115.61(15) 6_554 . ?
La9 La4 La7 91.74(3) . . ?
La6 La4 La7 59.21(3) 6_554 . ?
Ni2 La4 La4 49.00(4) . 12 ?
Ni3 La4 La4 108.86(5) . 12 ?
Mg1 La4 La4 114.09(14) . 12 ?
Mg2 La4 La4 148.38(12) 6_554 12 ?
La9 La4 La4 108.52(2) . 12 ?
La6 La4 La4 146.99(2) 6_554 12 ?
La7 La4 La4 90.79(2) . 12 ?
Ni2 La4 La3 108.83(5) . . ?
Ni3 La4 La3 48.97(5) . . ?
Mg1 La4 La3 113.94(14) . . ?
Mg2 La4 La3 147.80(12) 6_554 . ?
La9 La4 La3 147.11(3) . . ?
La6 La4 La3 108.22(3) 6_554 . ?
La7 La4 La3 59.72(3) . . ?
La4 La4 La3 60.131(18) 12 . ?
Ni2 La4 La12 52.17(7) . . ?
Ni3 La4 La12 110.97(5) . . ?
Mg1 La4 La12 149.45(13) . . ?
Mg2 La4 La12 116.44(15) 6_554 . ?
La9 La4 La12 60.03(3) . . ?
La6 La4 La12 90.85(3) 6_554 . ?
La7 La4 La12 60.68(3) . . ?
La4 La4 La12 60.217(17) 12 . ?
La3 La4 La12 89.85(3) . . ?
Ni2 La4 La8 48.74(5) . 16 ?
Ni3 La4 La8 155.10(5) . 16 ?
Mg1 La4 La8 57.56(13) . 16 ?
Mg2 La4 La8 57.72(12) 6_554 16 ?
La9 La4 La8 56.64(2) . 16 ?
La6 La4 La8 106.98(3) 6_554 16 ?
La7 La4 La8 146.90(3) . 16 ?
La4 La4 La8 90.665(19) 12 16 ?
La3 La4 La8 144.72(3) . 16 ?
La12 La4 La8 91.92(3) . 16 ?
Ni2 La4 La2 119.79(7) . . ?
Ni3 La4 La2 62.41(5) . . ?
Mg1 La4 La2 53.66(14) . . ?
Mg2 La4 La2 96.91(16) 6_554 . ?
La9 La4 La2 152.16(4) . . ?
La6 La4 La2 111.96(4) 6_554 . ?
La7 La4 La2 109.38(3) . . ?
La4 La4 La2 89.67(3) 12 . ?
La3 La4 La2 60.39(3) . . ?
La12 La4 La2 146.44(4) . . ?
La8 La4 La2 103.70(3) 16 . ?
Ni3 La5 Ni3 99.57(9) 5_455 16 ?
Ni3 La5 Ni5 94.90(6) 5_455 . ?
Ni3 La5 Ni5 94.90(6) 16 . ?
Ni3 La5 La6 66.94(5) 5_455 2_564 ?
Ni3 La5 La6 66.94(5) 16 2_564 ?
Ni5 La5 La6 150.24(7) . 2_564 ?
Ni3 La5 Mg1 151.49(16) 5_455 7 ?
Ni3 La5 Mg1 99.57(15) 16 7 ?
Ni5 La5 Mg1 104.30(11) . 7 ?
La6 La5 Mg1 101.95(8) 2_564 7 ?
Ni3 La5 Mg1 99.57(15) 5_455 5_455 ?
Ni3 La5 Mg1 151.49(17) 16 5_455 ?
Ni5 La5 Mg1 104.30(10) . 5_455 ?
La6 La5 Mg1 101.95(8) 2_564 5_455 ?
Mg1 La5 Mg1 55.6(3) 7 5_455 ?
Ni3 La5 Mg2 103.46(12) 5_455 2_564 ?
Ni3 La5 Mg2 103.46(12) 16 2_564 ?
Ni5 La5 Mg2 151.27(19) . 2_564 ?
La6 La5 Mg2 58.49(17) 2_564 2_564 ?
Mg1 La5 Mg2 51.33(18) 7 2_564 ?
Mg1 La5 Mg2 51.33(18) 5_455 2_564 ?
Ni3 La5 La5 123.48(5) 5_455 10_556 ?
Ni3 La5 La5 123.48(5) 16 10_556 ?
Ni5 La5 La5 51.08(6) . 10_556 ?
La6 La5 La5 158.67(3) 2_564 10_556 ?
Mg1 La5 La5 59.63(7) 7 10_556 ?
Mg1 La5 La5 59.63(7) 5_455 10_556 ?
Mg2 La5 La5 100.18(17) 2_564 10_556 ?
Ni3 La5 La2 153.31(6) 5_455 7 ?
Ni3 La5 La2 64.98(5) 16 7 ?
Ni5 La5 La2 66.57(3) . 7 ?
La6 La5 La2 120.09(2) 2_564 7 ?
Mg1 La5 La2 55.18(16) 7 7 ?
Mg1 La5 La2 103.49(13) 5_455 7 ?
Mg2 La5 La2 101.39(9) 2_564 7 ?
La5 La5 La2 60.36(2) 10_556 7 ?
Ni3 La5 La2 64.98(5) 5_455 5_455 ?
Ni3 La5 La2 153.31(6) 16 5_455 ?
Ni5 La5 La2 66.57(3) . 5_455 ?
La6 La5 La2 120.09(2) 2_564 5_455 ?
Mg1 La5 La2 103.49(13) 7 5_455 ?
Mg1 La5 La2 55.18(16) 5_455 5_455 ?
Mg2 La5 La2 101.39(9) 2_564 5_455 ?
La5 La5 La2 60.36(2) 10_556 5_455 ?
La2 La5 La2 119.07(4) 7 5_455 ?
Ni3 La5 La14 49.96(5) 5_455 . ?
Ni3 La5 La14 49.96(5) 16 . ?
Ni5 La5 La14 92.75(7) . . ?
La6 La5 La14 57.50(4) 2_564 . ?
Mg1 La5 La14 146.77(11) 7 . ?
Mg1 La5 La14 146.77(11) 5_455 . ?
Mg2 La5 La14 115.99(18) 2_564 . ?
La5 La5 La14 143.83(3) 10_556 . ?
La2 La5 La14 109.46(3) 7 . ?
La2 La5 La14 109.46(3) 5_455 . ?
Ni3 La5 La4 125.66(6) 5_455 16 ?
Ni3 La5 La4 48.40(4) 16 16 ?
Ni5 La5 La4 125.26(2) . 16 ?
La6 La5 La4 60.37(2) 2_564 16 ?
Mg1 La5 La4 57.65(10) 7 16 ?
Mg1 La5 La4 103.10(16) 5_455 16 ?
Mg2 La5 La4 59.15(6) 2_564 16 ?
La5 La5 La4 110.61(2) 10_556 16 ?
La2 La5 La4 61.42(2) 7 16 ?
La2 La5 La4 158.27(5) 5_455 16 ?
La14 La5 La4 89.20(3) . 16 ?
Ni4 La6 Ni4 102.18(10) 15_456 6 ?
Ni4 La6 Mg2 100.38(11) 15_456 . ?
Ni4 La6 Mg2 100.38(11) 6 . ?
Ni4 La6 La14 112.68(5) 15_456 2_565 ?
Ni4 La6 La14 112.68(5) 6 2_565 ?
Mg2 La6 La14 125.45(16) . 2_565 ?
Ni4 La6 La5 127.87(5) 15_456 2_565 ?
Ni4 La6 La5 127.87(5) 6 2_565 ?
Mg2 La6 La5 61.13(15) . 2_565 ?
La14 La6 La5 64.32(4) 2_565 2_565 ?
Ni4 La6 La15 70.24(5) 15_456 . ?
Ni4 La6 La15 70.24(5) 6 . ?
Mg2 La6 La15 164.10(16) . . ?
La14 La6 La15 70.45(4) 2_565 . ?
La5 La6 La15 134.77(5) 2_565 . ?
Ni4 La6 La13 51.20(5) 15_456 . ?
Ni4 La6 La13 51.20(5) 6 . ?
Mg2 La6 La13 102.80(15) . . ?
La14 La6 La13 131.75(5) 2_565 . ?
La5 La6 La13 163.93(5) 2_565 . ?
La15 La6 La13 61.30(4) . . ?
Ni4 La6 La7 131.73(6) 15_456 6 ?
Ni4 La6 La7 50.89(5) 6 6 ?
Mg2 La6 La7 121.43(4) . 6 ?
La14 La6 La7 63.05(3) 2_565 6 ?
La5 La6 La7 95.15(3) 2_565 6 ?
La15 La6 La7 63.21(3) . 6 ?
La13 La6 La7 93.72(3) . 6 ?
Ni4 La6 La7 50.89(5) 15_456 15_456 ?
Ni4 La6 La7 131.73(6) 6 15_456 ?
Mg2 La6 La7 121.43(4) . 15_456 ?
La14 La6 La7 63.05(3) 2_565 15_456 ?
La5 La6 La7 95.15(3) 2_565 15_456 ?
La15 La6 La7 63.21(2) . 15_456 ?
La13 La6 La7 93.72(3) . 15_456 ?
La7 La6 La7 112.82(5) 6 15_456 ?
Ni4 La6 La4 152.66(6) 15_456 6 ?
Ni4 La6 La4 65.36(5) 6 6 ?
Mg2 La6 La4 60.93(5) . 6 ?
La14 La6 La4 94.66(3) 2_565 6 ?
La5 La6 La4 63.24(2) 2_565 6 ?
La15 La6 La4 122.33(2) . 6 ?
La13 La6 La4 110.35(3) . 6 ?
La7 La6 La4 60.61(2) 6 6 ?
La7 La6 La4 155.01(4) 15_456 6 ?
Ni4 La6 La4 65.36(5) 15_456 15_456 ?
Ni4 La6 La4 152.66(6) 6 15_456 ?
Mg2 La6 La4 60.93(5) . 15_456 ?
La14 La6 La4 94.66(3) 2_565 15_456 ?
La5 La6 La4 63.24(2) 2_565 15_456 ?
La15 La6 La4 122.33(2) . 15_456 ?
La13 La6 La4 110.35(3) . 15_456 ?
La7 La6 La4 155.01(4) 6 15_456 ?
La7 La6 La4 60.61(2) 15_456 15_456 ?
La4 La6 La4 113.99(4) 6 15_456 ?
Ni4 La6 La9 46.42(5) 15_456 15_456 ?
Ni4 La6 La9 95.50(6) 6 15_456 ?
Mg2 La6 La9 56.17(12) . 15_456 ?
La14 La6 La9 149.372(18) 2_565 15_456 ?
La5 La6 La9 108.01(4) 2_565 15_456 ?
La15 La6 La9 110.77(4) . 15_456 ?
La13 La6 La9 58.65(3) . 15_456 ?
La7 La6 La9 146.37(4) 6 15_456 ?
La7 La6 La9 89.55(2) 15_456 15_456 ?
La4 La6 La9 108.37(4) 6 15_456 ?
La4 La6 La9 57.92(2) 15_456 15_456 ?
Ni4 La7 Ni1 150.80(7) . . ?
Ni4 La7 Ni3 102.33(6) . . ?
Ni1 La7 Ni3 101.10(8) . . ?
Ni4 La7 La6 48.98(5) . 6_554 ?
Ni1 La7 La6 160.19(6) . 6_554 ?
Ni3 La7 La6 64.47(5) . 6_554 ?
Ni4 La7 La9 160.75(5) . 16_545 ?
Ni1 La7 La9 48.36(5) . 16_545 ?
Ni3 La7 La9 64.29(5) . 16_545 ?
La6 La7 La9 111.83(3) 6_554 16_545 ?
Ni4 La7 La11 107.96(5) . . ?
Ni1 La7 La11 48.54(7) . . ?
Ni3 La7 La11 149.28(5) . . ?
La6 La7 La11 142.88(4) 6_554 . ?
La9 La7 La11 87.35(3) 16_545 . ?
Ni4 La7 La4 64.52(5) . . ?
Ni1 La7 La4 121.87(7) . . ?
Ni3 La7 La4 49.25(5) . . ?
La6 La7 La4 60.19(3) 6_554 . ?
La9 La7 La4 109.60(3) 16_545 . ?
La11 La7 La4 144.38(3) . . ?
Ni4 La7 La3 123.21(5) . . ?
Ni1 La7 La3 63.12(7) . . ?
Ni3 La7 La3 49.23(4) . . ?
La6 La7 La3 109.87(3) 6_554 . ?
La9 La7 La3 59.78(3) 16_545 . ?
La11 La7 La3 107.25(3) . . ?
La4 La7 La3 60.78(3) . . ?
Ni4 La7 La14 104.48(5) . 5_545 ?
Ni1 La7 La14 103.91(5) . 5_545 ?
Ni3 La7 La14 49.71(5) . 5_545 ?
La6 La7 La14 56.59(3) 6_554 5_545 ?
La9 La7 La14 56.46(3) 16_545 5_545 ?
La11 La7 La14 124.29(4) . 5_545 ?
La4 La7 La14 90.54(3) . 5_545 ?
La3 La7 La14 90.35(3) . 5_545 ?
Ni4 La7 La15 65.95(5) . 6_554 ?
Ni1 La7 La15 121.51(6) . 6_554 ?
Ni3 La7 La15 108.85(5) . 6_554 ?
La6 La7 La15 56.89(3) 6_554 6_554 ?
La9 La7 La15 103.96(3) 16_545 6_554 ?
La11 La7 La15 88.44(3) . 6_554 ?
La4 La7 La15 115.78(4) . 6_554 ?
La3 La7 La15 155.79(4) . 6_554 ?
La14 La7 La15 65.46(3) 5_545 6_554 ?
Ni4 La7 La12 48.64(5) . . ?
Ni1 La7 La12 106.82(5) . . ?
Ni3 La7 La12 108.87(5) . . ?
La6 La7 La12 91.26(3) 6_554 . ?
La9 La7 La12 146.54(3) 16_545 . ?
La11 La7 La12 87.95(3) . . ?
La4 La7 La12 60.41(3) . . ?
La3 La7 La12 90.30(3) . . ?
La14 La7 La12 145.76(4) 5_545 . ?
La15 La7 La12 109.01(3) 6_554 . ?
Ni4 La7 La10 47.78(5) . . ?
Ni1 La7 La10 109.08(7) . . ?
Ni3 La7 La10 149.54(5) . . ?
La6 La7 La10 87.00(3) 6_554 . ?
La9 La7 La10 142.15(3) 16_545 . ?
La11 La7 La10 61.17(3) . . ?
La4 La7 La10 108.25(3) . . ?
La3 La7 La10 145.70(3) . . ?
La14 La7 La10 123.35(3) 5_545 . ?
La15 La7 La10 58.16(3) 6_554 . ?
La12 La7 La10 58.76(3) . . ?
Ni5 La8 Ni3 95.23(9) 5_545 . ?
Ni5 La8 Ni2 95.19(6) 5_545 5_545 ?
Ni3 La8 Ni2 98.97(8) . 5_545 ?
Ni5 La8 La9 150.66(4) 5_545 16_545 ?
Ni3 La8 La9 67.30(5) . 16_545 ?
Ni2 La8 La9 66.26(5) 5_545 16_545 ?
Ni5 La8 Mg1 104.14(11) 5_545 7_545 ?
Ni3 La8 Mg1 151.37(17) . 7_545 ?
Ni2 La8 Mg1 100.04(15) 5_545 7_545 ?
La9 La8 Mg1 101.49(8) 16_545 7_545 ?
Ni5 La8 Mg3 104.40(10) 5_545 . ?
Ni3 La8 Mg3 99.6(2) . . ?
Ni2 La8 Mg3 151.5(2) 5_545 . ?
La9 La8 Mg3 101.77(5) 16_545 . ?
Mg1 La8 Mg3 55.4(3) 7_545 . ?
Ni5 La8 La8 50.98(3) 5_545 10_556 ?
Ni3 La8 La8 123.60(5) . 10_556 ?
Ni2 La8 La8 124.09(6) 5_545 10_556 ?
La9 La8 La8 158.36(2) 16_545 10_556 ?
Mg1 La8 La8 59.61(7) 7_545 10_556 ?
Mg3 La8 La8 59.691(15) . 10_556 ?
Ni5 La8 Mg2 151.15(17) 5_545 2_554 ?
Ni3 La8 Mg2 103.43(15) . 2_554 ?
Ni2 La8 Mg2 103.27(14) 5_545 2_554 ?
La9 La8 Mg2 58.18(17) 16_545 2_554 ?
Mg1 La8 Mg2 51.24(19) 7_545 2_554 ?
Mg3 La8 Mg2 51.2(2) . 2_554 ?
La8 La8 Mg2 100.18(17) 10_556 2_554 ?
Ni5 La8 La1 66.21(9) 5_545 5_545 ?
Ni3 La8 La1 153.18(5) . 5_545 ?
Ni2 La8 La1 65.55(6) 5_545 5_545 ?
La9 La8 La1 119.76(3) 16_545 5_545 ?
Mg1 La8 La1 55.43(16) 7_545 5_545 ?
Mg3 La8 La1 103.58(17) . 5_545 ?
La8 La8 La1 60.361(18) 10_556 5_545 ?
Mg2 La8 La1 101.51(13) 2_554 5_545 ?
Ni5 La8 La2 66.69(7) 5_545 . ?
Ni3 La8 La2 65.04(5) . . ?
Ni2 La8 La2 153.16(6) 5_545 . ?
La9 La8 La2 120.42(3) 16_545 . ?
Mg1 La8 La2 103.47(12) 7_545 . ?
Mg3 La8 La2 55.4(2) . . ?
La8 La8 La2 60.397(17) 10_556 . ?
Mg2 La8 La2 101.48(13) 2_554 . ?
La1 La8 La2 119.05(3) 5_545 . ?
Ni5 La8 La14 93.00(4) 5_545 5_545 ?
Ni3 La8 La14 50.02(5) . 5_545 ?
Ni2 La8 La14 49.33(7) 5_545 5_545 ?
La9 La8 La14 57.67(2) 16_545 5_545 ?
Mg1 La8 La14 146.66(11) 7_545 5_545 ?
Mg3 La8 La14 146.81(14) . 5_545 ?
La8 La8 La14 143.97(2) 10_556 5_545 ?
Mg2 La8 La14 115.85(17) 2_554 5_545 ?
La1 La8 La14 109.30(3) 5_545 5_545 ?
La2 La8 La14 109.58(3) . 5_545 ?
Ni5 La8 La4 125.12(8) 5_545 16_545 ?
Ni3 La8 La4 125.42(5) . 16_545 ?
Ni2 La8 La4 48.43(5) 5_545 16_545 ?
La9 La8 La4 59.81(2) 16_545 16_545 ?
Mg1 La8 La4 57.82(10) 7_545 16_545 ?
Mg3 La8 La4 103.1(2) . 16_545 ?
La8 La8 La4 110.725(18) 10_556 16_545 ?
Mg2 La8 La4 59.12(12) 2_554 16_545 ?
La1 La8 La4 61.61(3) 5_545 16_545 ?
La2 La8 La4 158.40(4) . 16_545 ?
La14 La8 La4 88.90(3) 5_545 16_545 ?
Ni1 La9 Ni4 102.32(8) 5 . ?
Ni1 La9 Mg2 99.24(11) 5 6_554 ?
Ni4 La9 Mg2 100.96(15) . 6_554 ?
Ni1 La9 La14 112.44(6) 5 . ?
Ni4 La9 La14 112.66(6) . . ?
Mg2 La9 La14 126.05(13) 6_554 . ?
Ni1 La9 La8 126.75(7) 5 16 ?
Ni4 La9 La8 128.92(6) . 16 ?
Mg2 La9 La8 61.71(13) 6_554 16 ?
La14 La9 La8 64.34(3) . 16 ?
Ni1 La9 La16 70.58(6) 5 16 ?
Ni4 La9 La16 68.46(5) . 16 ?
Mg2 La9 La16 162.33(13) 6_554 16 ?
La14 La9 La16 71.62(3) . 16 ?
La8 La9 La16 135.96(3) 16 16 ?
Ni1 La9 La4 152.76(6) 5 . ?
Ni4 La9 La4 66.13(5) . . ?
Mg2 La9 La4 61.48(10) 6_554 . ?
La14 La9 La4 94.77(3) . . ?
La8 La9 La4 63.55(3) 16 . ?
La16 La9 La4 122.00(3) 16 . ?
Ni1 La9 La13 51.52(7) 5 6_554 ?
Ni4 La9 La13 50.98(5) . 6_554 ?
Mg2 La9 La13 102.65(13) 6_554 6_554 ?
La14 La9 La13 131.30(4) . 6_554 ?
La8 La9 La13 164.35(4) 16 6_554 ?
La16 La9 La13 59.68(3) 16 6_554 ?
La4 La9 La13 110.88(3) . 6_554 ?
Ni1 La9 La7 50.71(6) 5 16 ?
Ni4 La9 La7 130.87(6) . 16 ?
Mg2 La9 La7 121.31(13) 6_554 16 ?
La14 La9 La7 62.78(3) . 16 ?
La8 La9 La7 94.87(3) 16 16 ?
La16 La9 La7 63.96(2) 16 16 ?
La4 La9 La7 154.92(3) . 16 ?
La13 La9 La7 93.21(3) 6_554 16 ?
Ni1 La9 La3 64.30(7) 5 5 ?
Ni4 La9 La3 152.66(6) . 5 ?
Mg2 La9 La3 60.84(13) 6_554 5 ?
La14 La9 La3 94.66(3) . 5 ?
La8 La9 La3 63.19(3) 16 5 ?
La16 La9 La3 122.73(3) 16 5 ?
La4 La9 La3 114.22(3) . 5 ?
La13 La9 La3 109.98(3) 6_554 5 ?
La7 La9 La3 60.60(3) 16 5 ?
Ni1 La9 La12 130.98(7) 5 . ?
Ni4 La9 La12 49.76(5) . . ?
Mg2 La9 La12 122.74(11) 6_554 . ?
La14 La9 La12 64.06(3) . . ?
La8 La9 La12 97.05(3) 16 . ?
La16 La9 La12 61.98(3) 16 . ?
La4 La9 La12 61.53(3) . . ?
La13 La9 La12 92.20(3) 6_554 . ?
La7 La9 La12 112.44(3) 16 . ?
La3 La9 La12 156.62(3) 5 . ?
Ni1 La9 La6 94.74(6) 5 6_554 ?
Ni4 La9 La6 46.71(5) . 6_554 ?
Mg2 La9 La6 56.48(15) 6_554 6_554 ?
La14 La9 La6 150.31(3) . 6_554 ?
La8 La9 La6 109.17(3) 16 6_554 ?
La16 La9 La6 108.80(3) 16 6_554 ?
La4 La9 La6 59.01(3) . 6_554 ?
La13 La9 La6 58.16(3) 6_554 6_554 ?
La7 La9 La6 145.46(3) 16 6_554 ?
La3 La9 La6 108.27(3) 5 6_554 ?
La12 La9 La6 89.41(3) . 6_554 ?
Ni6 La10 Ni4 110.00(9) . . ?
Ni6 La10 La16 53.36(7) . 16 ?
Ni4 La10 La16 68.43(5) . 16 ?
Ni6 La10 La10 123.22(8) . 13 ?
Ni4 La10 La10 126.53(6) . 13 ?
La16 La10 La10 151.00(4) 16 13 ?
Ni6 La10 La15 170.68(6) . 6_554 ?
Ni4 La10 La15 67.70(5) . 6_554 ?
La16 La10 La15 118.71(4) 16 6_554 ?
La10 La10 La15 60.57(3) 13 6_554 ?
Ni6 La10 La15 63.76(8) . 10_556 ?
Ni4 La10 La15 164.88(6) . 10_556 ?
La16 La10 La15 112.63(4) 16 10_556 ?
La10 La10 La15 60.16(3) 13 10_556 ?
La15 La10 La15 120.73(3) 6_554 10_556 ?
Ni6 La10 La13 111.65(7) . 6_554 ?
Ni4 La10 La13 50.48(5) . 6_554 ?
La16 La10 La13 59.68(3) 16 6_554 ?
La10 La10 La13 108.00(4) 13 6_554 ?
La15 La10 La13 59.63(3) 6_554 6_554 ?
La15 La10 La13 143.96(4) 10_556 6_554 ?
Ni6 La10 La12 69.54(7) . . ?
Ni4 La10 La12 49.54(5) . . ?
La16 La10 La12 62.15(3) 16 . ?
La10 La10 La12 146.83(5) 13 . ?
La15 La10 La12 112.31(4) 6_554 . ?
La15 La10 La12 116.61(3) 10_556 . ?
La13 La10 La12 91.70(3) 6_554 . ?
Ni6 La10 La16 51.28(6) . 13 ?
Ni4 La10 La16 129.47(5) . 13 ?
La16 La10 La16 64.28(3) 16 13 ?
La10 La10 La16 91.07(3) 13 13 ?
La15 La10 La16 122.54(3) 6_554 13 ?
La15 La10 La16 58.85(3) 10_556 13 ?
La13 La10 La16 89.60(3) 6_554 13 ?
La12 La10 La16 116.11(3) . 13 ?
Ni6 La10 La7 125.40(7) . . ?
Ni4 La10 La7 48.80(5) . . ?
La16 La10 La7 112.84(3) 16 . ?
La10 La10 La7 92.29(3) 13 . ?
La15 La10 La7 60.52(3) 6_554 . ?
La15 La10 La7 121.98(4) 10_556 . ?
La13 La10 La7 90.66(3) 6_554 . ?
La12 La10 La7 60.27(3) . . ?
La16 La10 La7 176.37(3) 13 . ?
Ni6 La10 La11 109.23(6) . 13 ?
Ni4 La10 La11 107.13(5) . 13 ?
La16 La10 La11 91.23(3) 16 13 ?
La10 La10 La11 61.59(3) 13 13 ?
La15 La10 La11 64.13(3) 6_554 13 ?
La15 La10 La11 87.99(3) 10_556 13 ?
La13 La10 La11 58.72(3) 6_554 13 ?
La12 La10 La11 148.53(4) . 13 ?
La16 La10 La11 58.41(3) 13 13 ?
La7 La10 La11 124.60(3) . 13 ?
Ni6 La10 La11 101.23(6) . . ?
Ni4 La10 La11 105.95(5) . . ?
La16 La10 La11 144.48(3) 16 . ?
La10 La10 La11 61.28(3) 13 . ?
La15 La10 La11 88.04(3) 6_554 . ?
La15 La10 La11 63.88(3) 10_556 . ?
La13 La10 La11 144.36(4) 6_554 . ?
La12 La10 La11 87.08(3) . . ?
La16 La10 La11 122.69(3) 13 . ?
La7 La10 La11 58.13(3) . . ?
La11 La10 La11 122.86(3) 13 . ?
Ni1 La11 Ni7 94.18(7) . 9 ?
Ni1 La11 Ni7 94.18(7) . . ?
Ni7 La11 Ni7 50.91(12) 9 . ?
Ni1 La11 La16 69.51(4) . 12 ?
Ni7 La11 La16 46.69(5) 9 12 ?
Ni7 La11 La16 92.83(6) . 12 ?
Ni1 La11 La16 69.51(4) . . ?
Ni7 La11 La16 92.83(6) 9 . ?
Ni7 La11 La16 46.69(5) . . ?
La16 La11 La16 117.59(5) 12 . ?
Ni1 La11 La13 138.87(8) . 10_556 ?
Ni7 La11 La13 49.69(3) 9 10_556 ?
Ni7 La11 La13 49.69(3) . 10_556 ?
La16 La11 La13 90.71(3) 12 10_556 ?
La16 La11 La13 90.71(3) . 10_556 ?
Ni1 La11 La7 50.33(5) . . ?
Ni7 La11 La7 141.37(5) 9 . ?
Ni7 La11 La7 109.57(5) . . ?
La16 La11 La7 115.96(4) 12 . ?
La16 La11 La7 63.24(2) . . ?
La13 La11 La7 148.725(18) 10_556 . ?
Ni1 La11 La7 50.33(5) . 12 ?
Ni7 La11 La7 109.57(5) 9 12 ?
Ni7 La11 La7 141.37(5) . 12 ?
La16 La11 La7 63.24(2) 12 12 ?
La16 La11 La7 115.96(4) . 12 ?
La13 La11 La7 148.725(18) 10_556 12 ?
La7 La11 La7 62.54(4) . 12 ?
Ni1 La11 La13 50.89(7) . 2_554 ?
Ni7 La11 La13 49.29(3) 9 2_554 ?
Ni7 La11 La13 49.29(3) . 2_554 ?
La16 La11 La13 58.86(2) 12 2_554 ?
La16 La11 La13 58.86(2) . 2_554 ?
La13 La11 La13 87.98(4) 10_556 2_554 ?
La7 La11 La13 92.19(3) . 2_554 ?
La7 La11 La13 92.19(3) 12 2_554 ?
Ni1 La11 La10 126.99(2) . 8_455 ?
Ni7 La11 La10 62.20(5) 9 8_455 ?
Ni7 La11 La10 102.47(6) . 8_455 ?
La16 La11 La10 59.82(2) 12 8_455 ?
La16 La11 La10 148.75(4) . 8_455 ?
La13 La11 La10 59.17(2) 10_556 8_455 ?
La7 La11 La10 147.93(4) . 8_455 ?
La7 La11 La10 91.34(2) 12 8_455 ?
La13 La11 La10 108.03(3) 2_554 8_455 ?
Ni1 La11 La10 126.99(2) . 13 ?
Ni7 La11 La10 102.47(6) 9 13 ?
Ni7 La11 La10 62.20(5) . 13 ?
La16 La11 La10 148.75(4) 12 13 ?
La16 La11 La10 59.82(2) . 13 ?
La13 La11 La10 59.17(2) 10_556 13 ?
La7 La11 La10 91.34(2) . 13 ?
La7 La11 La10 147.93(4) 12 13 ?
La13 La11 La10 108.03(3) 2_554 13 ?
La10 La11 La10 105.06(4) 8_455 13 ?
Ni1 La11 La10 110.38(6) . . ?
Ni7 La11 La10 154.39(5) 9 . ?
Ni7 La11 La10 117.64(6) . . ?
La16 La11 La10 149.10(4) 12 . ?
La16 La11 La10 89.25(2) . . ?
La13 La11 La10 104.80(4) 10_556 . ?
La7 La11 La10 60.70(3) . . ?
La7 La11 La10 92.26(3) 12 . ?
La13 La11 La10 146.13(2) 2_554 . ?
La10 La11 La10 105.41(3) 8_455 . ?
La10 La11 La10 57.14(3) 13 . ?
Ni4 La12 Ni4 154.44(10) 12 . ?
Ni4 La12 Ni2 100.14(5) 12 . ?
Ni4 La12 Ni2 100.14(5) . . ?
Ni4 La12 La9 157.50(6) 12 . ?
Ni4 La12 La9 48.06(5) . . ?
Ni2 La12 La9 62.39(3) . . ?
Ni4 La12 La9 48.06(5) 12 12 ?
Ni4 La12 La9 157.50(6) . 12 ?
Ni2 La12 La9 62.39(3) . 12 ?
La9 La12 La9 109.45(4) . 12 ?
Ni4 La12 La10 48.94(5) 12 12 ?
Ni4 La12 La10 111.33(6) . 12 ?
Ni2 La12 La10 148.409(18) . 12 ?
La9 La12 La10 144.39(4) . 12 ?
La9 La12 La10 87.63(2) 12 12 ?
Ni4 La12 La10 111.33(6) 12 . ?
Ni4 La12 La10 48.94(5) . . ?
Ni2 La12 La10 148.409(18) . . ?
La9 La12 La10 87.63(2) . . ?
La9 La12 La10 144.39(4) 12 . ?
La10 La12 La10 63.10(4) 12 . ?
Ni4 La12 La4 121.84(6) 12 . ?
Ni4 La12 La4 63.82(5) . . ?
Ni2 La12 La4 48.15(5) . . ?
La9 La12 La4 58.44(2) . . ?
La9 La12 La4 106.71(4) 12 . ?
La10 La12 La4 147.41(4) 12 . ?
La10 La12 La4 108.83(3) . . ?
Ni4 La12 La4 63.82(5) 12 12 ?
Ni4 La12 La4 121.84(6) . 12 ?
Ni2 La12 La4 48.15(5) . 12 ?
La9 La12 La4 106.71(4) . 12 ?
La9 La12 La4 58.44(2) 12 12 ?
La10 La12 La4 108.83(3) 12 12 ?
La10 La12 La4 147.41(4) . 12 ?
La4 La12 La4 59.57(3) . 12 ?
Ni4 La12 La7 49.09(5) 12 12 ?
Ni4 La12 La7 109.75(6) . 12 ?
Ni2 La12 La7 106.36(6) . 12 ?
La9 La12 La7 145.73(4) . 12 ?
La9 La12 La7 89.73(2) 12 12 ?
La10 La12 La7 60.98(3) 12 12 ?
La10 La12 La7 92.72(4) . 12 ?
La4 La12 La7 89.38(3) . 12 ?
La4 La12 La7 58.91(2) 12 12 ?
Ni4 La12 La7 109.75(6) 12 . ?
Ni4 La12 La7 49.09(5) . . ?
Ni2 La12 La7 106.36(6) . . ?
La9 La12 La7 89.73(2) . . ?
La9 La12 La7 145.73(4) 12 . ?
La10 La12 La7 92.72(4) 12 . ?
La10 La12 La7 60.98(3) . . ?
La4 La12 La7 58.91(2) . . ?
La4 La12 La7 89.38(3) 12 . ?
La7 La12 La7 61.20(4) 12 . ?
Ni4 La12 La16 121.60(6) 12 16 ?
Ni4 La12 La16 65.52(5) . 16 ?
Ni2 La12 La16 108.15(6) . 16 ?
La9 La12 La16 57.94(2) . 16 ?
La9 La12 La16 104.76(4) 12 16 ?
La10 La12 La16 88.01(3) 12 16 ?
La10 La12 La16 57.44(3) . 16 ?
La4 La12 La16 115.07(2) . 16 ?
La4 La12 La16 154.38(4) 12 16 ?
La7 La12 La16 145.46(4) 12 16 ?
La7 La12 La16 109.51(3) . 16 ?
Ni7 La13 Ni7 52.50(12) 2 10_556 ?
Ni7 La13 Ni4 154.93(8) 2 6 ?
Ni7 La13 Ni4 103.88(7) 10_556 6 ?
Ni7 La13 Ni4 103.88(7) 2 15_456 ?
Ni7 La13 Ni4 154.93(8) 10_556 15_456 ?
Ni4 La13 Ni4 97.67(9) 6 15_456 ?
Ni7 La13 Ni1 93.60(6) 2 2 ?
Ni7 La13 Ni1 93.60(6) 10_556 2 ?
Ni4 La13 Ni1 96.56(7) 6 2 ?
Ni4 La13 Ni1 96.56(7) 15_456 2 ?
Ni7 La13 La16 47.53(5) 2 2 ?
Ni7 La13 La16 95.23(7) 10_556 2 ?
Ni4 La13 La16 157.00(6) 6 2 ?
Ni4 La13 La16 67.42(5) 15_456 2 ?
Ni1 La13 La16 69.21(3) 2 2 ?
Ni7 La13 La16 95.23(6) 2 11_556 ?
Ni7 La13 La16 47.53(5) 10_556 11_556 ?
Ni4 La13 La16 67.42(5) 6 11_556 ?
Ni4 La13 La16 157.00(6) 15_456 11_556 ?
Ni1 La13 La16 69.21(3) 2 11_556 ?
La16 La13 La16 120.09(5) 2 11_556 ?
Ni7 La13 La6 151.89(6) 2 . ?
Ni7 La13 La6 151.89(6) 10_556 . ?
Ni4 La13 La6 48.93(5) 6 . ?
Ni4 La13 La6 48.93(5) 15_456 . ?
Ni1 La13 La6 96.42(7) 2 . ?
La16 La13 La6 112.87(3) 2 . ?
La16 La13 La6 112.87(3) 11_556 . ?
Ni7 La13 La15 109.44(4) 2 . ?
Ni7 La13 La15 109.44(4) 10_556 . ?
Ni4 La13 La15 67.36(5) 6 . ?
Ni4 La13 La15 67.36(5) 15_456 . ?
Ni1 La13 La15 154.21(8) 2 . ?
La16 La13 La15 118.19(2) 2 . ?
La16 La13 La15 118.19(2) 11_556 . ?
La6 La13 La15 57.79(4) . . ?
Ni7 La13 La9 138.41(5) 2 6 ?
Ni7 La13 La9 106.35(5) 10_556 6 ?
Ni4 La13 La9 48.42(5) 6 6 ?
Ni4 La13 La9 97.48(6) 15_456 6 ?
Ni1 La13 La9 48.30(5) 2 6 ?
La16 La13 La9 113.98(4) 2 6 ?
La16 La13 La9 59.52(2) 11_556 6 ?
La6 La13 La9 63.19(3) . 6 ?
La15 La13 La9 111.65(4) . 6 ?
Ni7 La13 La9 106.35(5) 2 15_456 ?
Ni7 La13 La9 138.41(5) 10_556 15_456 ?
Ni4 La13 La9 97.48(6) 6 15_456 ?
Ni4 La13 La9 48.42(5) 15_456 15_456 ?
Ni1 La13 La9 48.30(5) 2 15_456 ?
La16 La13 La9 59.52(2) 2 15_456 ?
La16 La13 La9 113.98(4) 11_556 15_456 ?
La6 La13 La9 63.19(3) . 15_456 ?
La15 La13 La9 111.65(4) . 15_456 ?
La9 La13 La9 63.64(4) 6 15_456 ?
Ni7 La13 La11 51.69(4) 2 10_556 ?
Ni7 La13 La11 51.69(3) 10_556 10_556 ?
Ni4 La13 La11 109.05(5) 6 10_556 ?
Ni4 La13 La11 109.05(5) 15_456 10_556 ?
Ni1 La13 La11 140.28(8) 2 10_556 ?
La16 La13 La11 92.78(3) 2 10_556 ?
La16 La13 La11 92.78(3) 11_556 10_556 ?
La6 La13 La11 123.30(5) . 10_556 ?
La15 La13 La11 65.51(4) . 10_556 ?
La9 La13 La11 148.157(18) 6 10_556 ?
La9 La13 La11 148.157(18) 15_456 10_556 ?
Ni2 La14 Ni3 97.30(7) . 16 ?
Ni2 La14 Ni3 97.30(7) . 5_455 ?
Ni3 La14 Ni3 96.88(9) 16 5_455 ?
Ni2 La14 La6 154.59(8) . 2_564 ?
Ni3 La14 La6 66.79(5) 16 2_564 ?
Ni3 La14 La6 66.79(5) 5_455 2_564 ?
Ni2 La14 La9 66.36(3) . 12 ?
Ni3 La14 La9 153.87(6) 16 12 ?
Ni3 La14 La9 66.91(4) 5_455 12 ?
La6 La14 La9 119.69(2) 2_564 12 ?
Ni2 La14 La9 66.36(3) . . ?
Ni3 La14 La9 66.91(4) 16 . ?
Ni3 La14 La9 153.87(6) 5_455 . ?
La6 La14 La9 119.69(2) 2_564 . ?
La9 La14 La9 119.08(5) 12 . ?
Ni2 La14 La8 49.09(5) . 16 ?
Ni3 La14 La8 48.57(5) 16 16 ?
Ni3 La14 La8 95.88(5) 5_455 16 ?
La6 La14 La8 110.64(4) 2_564 16 ?
La9 La14 La8 110.50(4) 12 16 ?
La9 La14 La8 57.99(2) . 16 ?
Ni2 La14 La8 49.09(5) . 5_455 ?
Ni3 La14 La8 95.88(5) 16 5_455 ?
Ni3 La14 La8 48.57(5) 5_455 5_455 ?
La6 La14 La8 110.64(4) 2_564 5_455 ?
La9 La14 La8 57.99(2) 12 5_455 ?
La9 La14 La8 110.50(4) . 5_455 ?
La8 La14 La8 61.40(3) 16 5_455 ?
Ni2 La14 La7 125.42(2) . 16 ?
Ni3 La14 La7 50.39(4) 16 16 ?
Ni3 La14 La7 125.30(6) 5_455 16 ?
La6 La14 La7 60.35(2) 2_564 16 ?
La9 La14 La7 155.73(4) 12 16 ?
La9 La14 La7 60.76(2) . 16 ?
La8 La14 La7 90.14(2) 16 16 ?
La8 La14 La7 146.27(4) 5_455 16 ?
Ni2 La14 La7 125.42(2) . 5_455 ?
Ni3 La14 La7 125.30(6) 16 5_455 ?
Ni3 La14 La7 50.39(4) 5_455 5_455 ?
La6 La14 La7 60.35(2) 2_564 5_455 ?
La9 La14 La7 60.76(2) 12 5_455 ?
La9 La14 La7 155.73(4) . 5_455 ?
La8 La14 La7 146.27(4) 16 5_455 ?
La8 La14 La7 90.14(2) 5_455 5_455 ?
La7 La14 La7 108.61(4) 16 5_455 ?
Ni2 La14 La5 96.41(7) . . ?
Ni3 La14 La5 48.61(5) 16 . ?
Ni3 La14 La5 48.61(5) 5_455 . ?
La6 La14 La5 58.18(4) 2_564 . ?
La9 La14 La5 110.66(3) 12 . ?
La9 La14 La5 110.66(3) . . ?
La8 La14 La5 61.28(3) 16 . ?
La8 La14 La5 61.28(3) 5_455 . ?
La7 La14 La5 90.12(3) 16 . ?
La7 La14 La5 90.12(3) 5_455 . ?
Ni2 La14 La12 51.13(7) . . ?
Ni3 La14 La12 125.92(5) 16 . ?
Ni3 La14 La12 125.92(5) 5_455 . ?
La6 La14 La12 154.28(5) 2_564 . ?
La9 La14 La12 60.46(2) 12 . ?
La9 La14 La12 60.46(2) . . ?
La8 La14 La12 91.31(3) 16 . ?
La8 La14 La12 91.31(3) 5_455 . ?
La7 La14 La12 108.14(3) 16 . ?
La7 La14 La12 108.14(3) 5_455 . ?
La5 La14 La12 147.54(5) . . ?
Ni6 La15 La6 155.94(7) 10_556 . ?
Ni6 La15 La16 48.56(5) 10_556 6 ?
La6 La15 La16 112.08(4) . 6 ?
Ni6 La15 La16 48.56(5) 10_556 15_456 ?
La6 La15 La16 112.08(4) . 15_456 ?
La16 La15 La16 59.74(4) 6 15_456 ?
Ni6 La15 La13 143.15(7) 10_556 . ?
La6 La15 La13 60.91(4) . . ?
La16 La15 La13 149.956(19) 6 . ?
La16 La15 La13 149.96(2) 15_456 . ?
Ni6 La15 La10 102.86(4) 10_556 15_456 ?
La6 La15 La10 90.63(3) . 15_456 ?
La16 La15 La10 148.30(4) 6 15_456 ?
La16 La15 La10 91.89(2) 15_456 15_456 ?
La13 La15 La10 60.43(3) . 15_456 ?
Ni6 La15 La10 102.86(4) 10_556 6 ?
La6 La15 La10 90.63(3) . 6 ?
La16 La15 La10 91.89(2) 6 6 ?
La16 La15 La10 148.30(4) 15_456 6 ?
La13 La15 La10 60.43(3) . 6 ?
La10 La15 La10 110.37(5) 15_456 6 ?
Ni6 La15 La10 44.06(4) 10_556 3 ?
La6 La15 La10 147.30(2) . 3 ?
La16 La15 La10 92.36(4) 6 3 ?
La16 La15 La10 61.12(3) 15_456 3 ?
La13 La15 La10 107.61(4) . 3 ?
La10 La15 La10 59.27(3) 15_456 3 ?
La10 La15 La10 110.67(4) 6 3 ?
Ni6 La15 La10 44.06(4) 10_556 10_556 ?
La6 La15 La10 147.30(2) . 10_556 ?
La16 La15 La10 61.12(3) 6 10_556 ?
La16 La15 La10 92.36(4) 15_456 10_556 ?
La13 La15 La10 107.61(4) . 10_556 ?
La10 La15 La10 110.67(4) 15_456 10_556 ?
La10 La15 La10 59.27(3) 6 10_556 ?
La10 La15 La10 63.51(4) 3 10_556 ?
Ni6 La15 La7 109.34(4) 10_556 6 ?
La6 La15 La7 59.90(3) . 6 ?
La16 La15 La7 62.83(2) 6 6 ?
La16 La15 La7 110.34(4) 15_456 6 ?
La13 La15 La7 91.60(3) . 6 ?
La10 La15 La7 147.77(5) 15_456 6 ?
La10 La15 La7 61.33(2) 6 6 ?
La10 La15 La7 152.23(4) 3 6 ?
La10 La15 La7 92.01(2) 10_556 6 ?
Ni6 La15 La7 109.34(4) 10_556 15_456 ?
La6 La15 La7 59.90(3) . 15_456 ?
La16 La15 La7 110.34(4) 6 15_456 ?
La16 La15 La7 62.83(2) 15_456 15_456 ?
La13 La15 La7 91.60(3) . 15_456 ?
La10 La15 La7 61.33(2) 15_456 15_456 ?
La10 La15 La7 147.77(5) 6 15_456 ?
La10 La15 La7 92.01(2) 3 15_456 ?
La10 La15 La7 152.23(4) 10_556 15_456 ?
La7 La15 La7 107.68(5) 6 15_456 ?
Ni6 La15 La11 85.75(6) 10_556 10_556 ?
La6 La15 La11 118.31(5) . 10_556 ?
La16 La15 La11 120.65(4) 6 10_556 ?
La16 La15 La11 120.65(4) 15_456 10_556 ?
La13 La15 La11 57.40(3) . 10_556 ?
La10 La15 La11 59.48(3) 15_456 10_556 ?
La10 La15 La11 59.48(3) 6 10_556 ?
La10 La15 La11 59.56(3) 3 10_556 ?
La10 La15 La11 59.56(3) 10_556 10_556 ?
La7 La15 La11 120.77(3) 6 10_556 ?
La7 La15 La11 120.77(3) 15_456 10_556 ?
Ni7 La16 Ni6 87.24(7) . 13 ?
Ni7 La16 Ni6 87.14(7) . 5_545 ?
Ni6 La16 Ni6 49.66(11) 13 5_545 ?
Ni7 La16 La10 67.07(3) . 16_545 ?
Ni6 La16 La10 92.70(7) 13 16_545 ?
Ni6 La16 La10 47.40(5) 5_545 16_545 ?
Ni7 La16 La9 111.20(5) . 16_545 ?
Ni6 La16 La9 161.04(5) 13 16_545 ?
Ni6 La16 La9 124.19(7) 5_545 16_545 ?
La10 La16 La9 90.67(3) 16_545 16_545 ?
Ni7 La16 La13 51.17(5) . 2_554 ?
Ni6 La16 La13 136.22(6) 13 2_554 ?
Ni6 La16 La13 107.62(5) 5_545 2_554 ?
La10 La16 La13 61.48(3) 16_545 2_554 ?
La9 La16 La13 60.80(3) 16_545 2_554 ?
Ni7 La16 La16 133.94(5) . 12_655 ?
Ni6 La16 La16 51.75(4) 13 12_655 ?
Ni6 La16 La16 51.83(4) 5_545 12_655 ?
La10 La16 La16 92.01(2) 16_545 12_655 ?
La9 La16 La16 109.50(2) 16_545 12_655 ?
La13 La16 La16 150.05(2) 2_554 12_655 ?
Ni7 La16 La15 123.72(4) . 6_554 ?
Ni6 La16 La15 62.71(7) 13 6_554 ?
Ni6 La16 La15 103.21(5) 5_545 6_554 ?
La10 La16 La15 150.29(3) 16_545 6_554 ?
La9 La16 La15 107.50(4) 16_545 6_554 ?
La13 La16 La15 148.07(4) 2_554 6_554 ?
La16 La16 La15 60.132(19) 12_655 6_554 ?
Ni7 La16 La11 52.26(5) . . ?
Ni6 La16 La11 107.16(5) 13 . ?
Ni6 La16 La11 136.76(6) 5_545 . ?
La10 La16 La11 113.73(3) 16_545 . ?
La9 La16 La11 88.43(3) 16_545 . ?
La13 La16 La11 61.03(3) 2_554 . ?
La16 La16 La11 148.80(2) 12_655 . ?
La15 La16 La11 90.62(3) 6_554 . ?
Ni7 La16 La10 64.91(3) . 13 ?
Ni6 La16 La10 45.81(5) 13 13 ?
Ni6 La16 La10 89.97(7) 5_545 13 ?
La10 La16 La10 115.57(3) 16_545 13 ?
La9 La16 La10 145.82(3) 16_545 13 ?
La13 La16 La10 111.36(3) 2_554 13 ?
La16 La16 La10 91.94(2) 12_655 13 ?
La15 La16 La10 60.03(3) 6_554 13 ?
La11 La16 La10 61.77(3) . 13 ?
Ni7 La16 La12 126.09(4) . 5_545 ?
Ni6 La16 La12 105.92(5) 13 5_545 ?
Ni6 La16 La12 66.55(7) 5_545 5_545 ?
La10 La16 La12 60.42(3) 16_545 5_545 ?
La9 La16 La12 60.09(2) 16_545 5_545 ?
La13 La16 La12 91.73(3) 2_554 5_545 ?
La16 La16 La12 61.241(17) 12_655 5_545 ?
La15 La16 La12 108.19(3) 6_554 5_545 ?
La11 La16 La12 146.67(3) . 5_545 ?
La10 La16 La12 151.55(3) 13 5_545 ?
Ni7 La16 La7 110.53(5) . . ?
Ni6 La16 La7 120.20(7) 13 . ?
Ni6 La16 La7 160.30(5) 5_545 . ?
La10 La16 La7 147.09(3) 16_545 . ?
La9 La16 La7 58.66(2) 16_545 . ?
La13 La16 La7 90.75(3) 2_554 . ?
La16 La16 La7 108.483(19) 12_655 . ?
La15 La16 La7 60.11(3) 6_554 . ?
La11 La16 La7 58.64(3) . . ?
La10 La16 La7 89.85(3) 13 . ?
La12 La16 La7 106.82(3) 5_545 . ?
La9 Ni1 La9 88.18(9) 16_545 5_445 ?
La9 Ni1 La11 131.43(7) 16_545 . ?
La9 Ni1 La11 131.43(7) 5_445 . ?
La9 Ni1 La7 80.92(5) 16_545 . ?
La9 Ni1 La7 140.31(12) 5_445 . ?
La11 Ni1 La7 81.13(7) . . ?
La9 Ni1 La7 140.31(12) 16_545 12 ?
La9 Ni1 La7 80.92(5) 5_445 12 ?
La11 Ni1 La7 81.13(7) . 12 ?
La7 Ni1 La7 83.57(9) . 12 ?
La9 Ni1 La13 80.17(7) 16_545 2_554 ?
La9 Ni1 La13 80.17(7) 5_445 2_554 ?
La11 Ni1 La13 80.85(9) . 2_554 ?
La7 Ni1 La13 134.09(6) . 2_554 ?
La7 Ni1 La13 134.09(6) 12 2_554 ?
La9 Ni1 La3 70.34(7) 16_545 . ?
La9 Ni1 La3 70.34(7) 5_445 . ?
La11 Ni1 La3 140.82(11) . . ?
La7 Ni1 La3 70.04(7) . . ?
La7 Ni1 La3 70.04(7) 12 . ?
La13 Ni1 La3 138.33(11) 2_554 . ?
La4 Ni2 La4 82.00(9) 12 . ?
La4 Ni2 La8 138.78(12) 12 16 ?
La4 Ni2 La8 82.83(5) . 16 ?
La4 Ni2 La8 82.83(5) 12 5_455 ?
La4 Ni2 La8 138.78(12) . 5_455 ?
La8 Ni2 La8 83.87(9) 16 5_455 ?
La4 Ni2 La14 134.16(7) 12 . ?
La4 Ni2 La14 134.16(7) . . ?
La8 Ni2 La14 81.58(7) 16 . ?
La8 Ni2 La14 81.58(7) 5_455 . ?
La4 Ni2 La12 79.69(7) 12 . ?
La4 Ni2 La12 79.69(7) . . ?
La8 Ni2 La12 134.26(6) 16 . ?
La8 Ni2 La12 134.26(6) 5_455 . ?
La14 Ni2 La12 81.10(9) . . ?
La8 Ni3 La5 84.43(6) . 5_545 ?
La8 Ni3 La4 139.86(8) . . ?
La5 Ni3 La4 83.39(6) 5_545 . ?
La8 Ni3 La3 83.07(6) . . ?
La5 Ni3 La3 139.98(9) 5_545 . ?
La4 Ni3 La3 82.16(6) . . ?
La8 Ni3 La14 81.41(6) . 5_545 ?
La5 Ni3 La14 81.44(6) 5_545 5_545 ?
La4 Ni3 La14 133.78(8) . 5_545 ?
La3 Ni3 La14 133.42(8) . 5_545 ?
La8 Ni3 La7 133.52(8) . . ?
La5 Ni3 La7 133.43(8) 5_545 . ?
La4 Ni3 La7 79.63(6) . . ?
La3 Ni3 La7 79.77(6) . . ?
La14 Ni3 La7 79.90(6) 5_545 . ?
La9 Ni4 La6 86.87(7) . 6_554 ?
La9 Ni4 La10 132.43(9) . . ?
La6 Ni4 La10 131.42(9) 6_554 . ?
La9 Ni4 La12 82.18(7) . . ?
La6 Ni4 La12 139.71(9) 6_554 . ?
La10 Ni4 La12 81.52(6) . . ?
La9 Ni4 La7 137.55(8) . . ?
La6 Ni4 La7 80.14(6) 6_554 . ?
La10 Ni4 La7 83.43(6) . . ?
La12 Ni4 La7 82.27(6) . . ?
La9 Ni4 La13 80.61(6) . 6_554 ?
La6 Ni4 La13 79.87(6) 6_554 6_554 ?
La10 Ni4 La13 80.45(6) . 6_554 ?
La12 Ni4 La13 135.33(9) . 6_554 ?
La7 Ni4 La13 135.08(9) . 6_554 ?
La8 Ni5 La8 134.68(17) 5_455 7 ?
La8 Ni5 La8 84.85(7) 5_455 16 ?
La8 Ni5 La8 78.05(7) 7 16 ?
La8 Ni5 La8 78.05(7) 5_455 14_456 ?
La8 Ni5 La8 84.85(7) 7 14_456 ?
La8 Ni5 La8 134.68(17) 16 14_456 ?
La8 Ni5 La5 134.05(8) 5_455 10_556 ?
La8 Ni5 La5 84.50(4) 7 10_556 ?
La8 Ni5 La5 134.05(8) 16 10_556 ?
La8 Ni5 La5 84.50(4) 14_456 10_556 ?
La8 Ni5 La5 84.50(4) 5_455 . ?
La8 Ni5 La5 134.05(8) 7 . ?
La8 Ni5 La5 84.50(4) 16 . ?
La8 Ni5 La5 134.05(8) 14_456 . ?
La5 Ni5 La5 77.83(12) 10_556 . ?
Ni6 Ni6 La10 133.76(5) 9_565 12 ?
Ni6 Ni6 La10 133.76(5) 9_565 . ?
La10 Ni6 La10 92.19(10) 12 . ?
Ni6 Ni6 La16 65.28(11) 9_565 8_455 ?
La10 Ni6 La16 82.90(5) 12 8_455 ?
La10 Ni6 La16 140.22(13) . 8_455 ?
Ni6 Ni6 La16 65.28(11) 9_565 13 ?
La10 Ni6 La16 140.22(13) 12 13 ?
La10 Ni6 La16 82.90(5) . 13 ?
La16 Ni6 La16 76.49(9) 8_455 13 ?
Ni6 Ni6 La16 65.06(11) 9_565 16 ?
La10 Ni6 La16 134.72(13) 12 16 ?
La10 Ni6 La16 79.23(5) . 16 ?
La16 Ni6 La16 130.34(11) 8_455 16 ?
La16 Ni6 La16 83.24(6) 13 16 ?
Ni6 Ni6 La16 65.06(11) 9_565 5_455 ?
La10 Ni6 La16 79.23(5) 12 5_455 ?
La10 Ni6 La16 134.72(13) . 5_455 ?
La16 Ni6 La16 83.24(6) 8_455 5_455 ?
La16 Ni6 La16 130.34(11) 13 5_455 ?
La16 Ni6 La16 76.33(9) 16 5_455 ?
Ni6 Ni6 La15 120.32(19) 9_565 10_556 ?
La10 Ni6 La15 72.18(7) 12 10_556 ?
La10 Ni6 La15 72.18(7) . 10_556 ?
La16 Ni6 La15 68.73(7) 8_455 10_556 ?
La16 Ni6 La15 68.73(7) 13 10_556 ?
La16 Ni6 La15 141.78(5) 16 10_556 ?
La16 Ni6 La15 141.78(5) 5_455 10_556 ?
Ni7 Ni7 La16 133.94(5) 9 4 ?
Ni7 Ni7 La16 133.94(5) 9 . ?
La16 Ni7 La16 92.11(11) 4 . ?
Ni7 Ni7 La13 63.75(6) 9 10_556 ?
La16 Ni7 La13 81.30(3) 4 10_556 ?
La16 Ni7 La13 139.92(5) . 10_556 ?
Ni7 Ni7 La13 63.75(6) 9 2_554 ?
La16 Ni7 La13 139.92(5) 4 2_554 ?
La16 Ni7 La13 81.30(3) . 2_554 ?
La13 Ni7 La13 127.50(12) 10_556 2_554 ?
Ni7 Ni7 La11 64.54(6) 9 9 ?
La16 Ni7 La11 81.04(3) 4 9 ?
La16 Ni7 La11 138.78(5) . 9 ?
La13 Ni7 La11 79.46(6) 10_556 9 ?
La13 Ni7 La11 78.62(6) 2_554 9 ?
Ni7 Ni7 La11 64.54(6) 9 . ?
La16 Ni7 La11 138.78(5) 4 . ?
La16 Ni7 La11 81.04(3) . . ?
La13 Ni7 La11 78.62(6) 10_556 . ?
La13 Ni7 La11 79.46(6) 2_554 . ?
La11 Ni7 La11 129.09(12) 9 . ?
Mg2 Mg1 Mg2 103.7(4) 13_556 6_554 ?
Mg2 Mg1 Mg3 57.8(2) 13_556 5 ?
Mg2 Mg1 Mg3 57.8(2) 6_554 5 ?
Mg2 Mg1 Mg1 57.54(18) 13_556 3_655 ?
Mg2 Mg1 Mg1 57.54(18) 6_554 3_655 ?
Mg3 Mg1 Mg1 59.9(2) 5 3_655 ?
Mg2 Mg1 La2 120.8(2) 13_556 . ?
Mg2 Mg1 La2 120.8(2) 6_554 . ?
Mg3 Mg1 La2 176.2(3) 5 . ?
Mg1 Mg1 La2 116.28(15) 3_655 . ?
Mg2 Mg1 La1 121.05(19) 13_556 . ?
Mg2 Mg1 La1 121.05(19) 6_554 . ?
Mg3 Mg1 La1 116.4(3) 5 . ?
Mg1 Mg1 La1 176.28(15) 3_655 . ?
La2 Mg1 La1 67.44(19) . . ?
Mg2 Mg1 La8 65.24(15) 13_556 7 ?
Mg2 Mg1 La8 112.1(3) 6_554 7 ?
Mg3 Mg1 La8 62.41(17) 5 7 ?
Mg1 Mg1 La8 113.39(16) 3_655 7 ?
La2 Mg1 La8 120.7(2) . 7 ?
La1 Mg1 La8 63.52(14) . 7 ?
Mg2 Mg1 La8 112.1(3) 13_556 16 ?
Mg2 Mg1 La8 65.24(15) 6_554 16 ?
Mg3 Mg1 La8 62.41(17) 5 16 ?
Mg1 Mg1 La8 113.39(16) 3_655 16 ?
La2 Mg1 La8 120.7(2) . 16 ?
La1 Mg1 La8 63.52(14) . 16 ?
La8 Mg1 La8 60.78(13) 7 16 ?
Mg2 Mg1 La5 111.7(3) 13_556 5_545 ?
Mg2 Mg1 La5 64.76(18) 6_554 5_545 ?
Mg3 Mg1 La5 113.2(3) 5 5_545 ?
Mg1 Mg1 La5 62.19(16) 3_655 5_545 ?
La2 Mg1 La5 63.63(14) . 5_545 ?
La1 Mg1 La5 120.8(2) . 5_545 ?
La8 Mg1 La5 175.4(3) 7 5_545 ?
La8 Mg1 La5 119.02(3) 16 5_545 ?
Mg2 Mg1 La5 64.76(18) 13_556 14_546 ?
Mg2 Mg1 La5 111.7(3) 6_554 14_546 ?
Mg3 Mg1 La5 113.2(3) 5 14_546 ?
Mg1 Mg1 La5 62.19(16) 3_655 14_546 ?
La2 Mg1 La5 63.63(14) . 14_546 ?
La1 Mg1 La5 120.8(2) . 14_546 ?
La8 Mg1 La5 119.02(3) 7 14_546 ?
La8 Mg1 La5 175.4(3) 16 14_546 ?
La5 Mg1 La5 60.75(13) 5_545 14_546 ?
Mg2 Mg1 La4 170.0(3) 13_556 . ?
Mg2 Mg1 La4 66.23(14) 6_554 . ?
Mg3 Mg1 La4 114.07(14) 5 . ?
Mg1 Mg1 La4 114.09(14) 3_655 . ?
La2 Mg1 La4 66.97(15) . . ?
La1 Mg1 La4 66.91(15) . . ?
La8 Mg1 La4 117.6(2) 7 . ?
La8 Mg1 La4 64.62(9) 16 . ?
La5 Mg1 La4 64.79(8) 5_545 . ?
La5 Mg1 La4 117.8(2) 14_546 . ?
Mg2 Mg1 La4 66.23(14) 13_556 10_556 ?
Mg2 Mg1 La4 170.0(3) 6_554 10_556 ?
Mg3 Mg1 La4 114.07(14) 5 10_556 ?
Mg1 Mg1 La4 114.09(14) 3_655 10_556 ?
La2 Mg1 La4 66.97(15) . 10_556 ?
La1 Mg1 La4 66.91(15) . 10_556 ?
La8 Mg1 La4 64.62(9) 7 10_556 ?
La8 Mg1 La4 117.6(2) 16 10_556 ?
La5 Mg1 La4 117.8(2) 5_545 10_556 ?
La5 Mg1 La4 64.79(8) 14_546 10_556 ?
La4 Mg1 La4 123.8(3) . 10_556 ?
Mg1 Mg2 Mg1 64.9(4) 13_556 15_456 ?
Mg1 Mg2 Mg3 64.6(3) 13_556 9_556 ?
Mg1 Mg2 Mg3 64.6(3) 15_456 9_556 ?
Mg1 Mg2 La9 178.1(3) 13_556 15_456 ?
Mg1 Mg2 La9 113.44(15) 15_456 15_456 ?
Mg3 Mg2 La9 113.9(3) 9_556 15_456 ?
Mg1 Mg2 La9 113.44(15) 13_556 6 ?
Mg1 Mg2 La9 178.1(3) 15_456 6 ?
Mg3 Mg2 La9 113.9(3) 9_556 6 ?
La9 Mg2 La9 68.18(19) 15_456 6 ?
Mg1 Mg2 La6 114.1(3) 13_556 . ?
Mg1 Mg2 La6 114.1(3) 15_456 . ?
Mg3 Mg2 La6 178.4(4) 9_556 . ?
La9 Mg2 La6 67.34(19) 15_456 . ?
La9 Mg2 La6 67.34(19) 6 . ?
Mg1 Mg2 La5 63.9(2) 13_556 2_565 ?
Mg1 Mg2 La5 63.9(2) 15_456 2_565 ?
Mg3 Mg2 La5 118.0(4) 9_556 2_565 ?
La9 Mg2 La5 116.5(2) 15_456 2_565 ?
La9 Mg2 La5 116.5(2) 6 2_565 ?
La6 Mg2 La5 60.38(14) . 2_565 ?
Mg1 Mg2 La8 118.0(3) 13_556 2 ?
Mg1 Mg2 La8 63.52(18) 15_456 2 ?
Mg3 Mg2 La8 63.67(15) 9_556 2 ?
La9 Mg2 La8 60.11(8) 15_456 2 ?
La9 Mg2 La8 117.2(2) 6 2 ?
La6 Mg2 La8 116.81(17) . 2 ?
La5 Mg2 La8 116.97(14) 2_565 2 ?
Mg1 Mg2 La8 63.52(18) 13_556 11_556 ?
Mg1 Mg2 La8 118.0(3) 15_456 11_556 ?
Mg3 Mg2 La8 63.67(15) 9_556 11_556 ?
La9 Mg2 La8 117.2(2) 15_456 11_556 ?
La9 Mg2 La8 60.11(8) 6 11_556 ?
La6 Mg2 La8 116.81(17) . 11_556 ?
La5 Mg2 La8 116.97(14) 2_565 11_556 ?
La8 Mg2 La8 116.9(2) 2 11_556 ?
Mg1 Mg2 La3 116.9(3) 13_556 2 ?
Mg1 Mg2 La3 116.9(3) 15_456 2 ?
Mg3 Mg2 La3 62.9(3) 9_556 2 ?
La9 Mg2 La3 62.70(14) 15_456 2 ?
La9 Mg2 La3 62.70(14) 6 2 ?
La6 Mg2 La3 118.7(3) . 2 ?
La5 Mg2 La3 179.0(3) 2_565 2 ?
La8 Mg2 La3 63.31(12) 2 2 ?
La8 Mg2 La3 63.31(12) 11_556 2 ?
Mg1 Mg2 La4 63.04(17) 13_556 6 ?
Mg1 Mg2 La4 117.4(3) 15_456 6 ?
Mg3 Mg2 La4 116.98(18) 9_556 6 ?
La9 Mg2 La4 118.9(3) 15_456 6 ?
La9 Mg2 La4 61.87(10) 6 6 ?
La6 Mg2 La4 62.56(13) . 6 ?
La5 Mg2 La4 63.57(12) 2_565 6 ?
La8 Mg2 La4 179.0(3) 2 6 ?
La8 Mg2 La4 63.16(2) 11_556 6 ?
La3 Mg2 La4 116.13(14) 2 6 ?
Mg1 Mg2 La4 117.4(3) 13_556 15_456 ?
Mg1 Mg2 La4 63.04(17) 15_456 15_456 ?
Mg3 Mg2 La4 116.98(18) 9_556 15_456 ?
La9 Mg2 La4 61.87(10) 15_456 15_456 ?
La9 Mg2 La4 118.9(3) 6 15_456 ?
La6 Mg2 La4 62.56(13) . 15_456 ?
La5 Mg2 La4 63.57(12) 2_565 15_456 ?
La8 Mg2 La4 63.16(2) 2 15_456 ?
La8 Mg2 La4 179.0(3) 11_556 15_456 ?
La3 Mg2 La4 116.13(14) 2 15_456 ?
La4 Mg2 La4 116.8(2) 6 15_456 ?
Mg2 Mg3 Mg2 103.6(5) 2_554 9_556 ?
Mg2 Mg3 Mg1 57.6(3) 2_554 5_445 ?
Mg2 Mg3 Mg1 57.6(3) 9_556 5_445 ?
Mg2 Mg3 Mg1 57.6(3) 2_554 7_545 ?
Mg2 Mg3 Mg1 57.6(3) 9_556 7_545 ?
Mg1 Mg3 Mg1 60.2(4) 5_445 7_545 ?
Mg2 Mg3 La2 120.95(16) 2_554 . ?
Mg2 Mg3 La2 120.95(16) 9_556 . ?
Mg1 Mg3 La2 176.3(3) 5_445 . ?
Mg1 Mg3 La2 116.10(15) 7_545 . ?
Mg2 Mg3 La2 120.95(16) 2_554 3 ?
Mg2 Mg3 La2 120.95(16) 9_556 3 ?
Mg1 Mg3 La2 116.10(15) 5_445 3 ?
Mg1 Mg3 La2 176.3(3) 7_545 3 ?
La2 Mg3 La2 67.6(3) . 3 ?
Mg2 Mg3 La3 169.6(5) 2_554 10_556 ?
Mg2 Mg3 La3 66.07(17) 9_556 10_556 ?
Mg1 Mg3 La3 113.83(15) 5_445 10_556 ?
Mg1 Mg3 La3 113.83(15) 7_545 10_556 ?
La2 Mg3 La3 67.2(2) . 10_556 ?
La2 Mg3 La3 67.2(2) 3 10_556 ?
Mg2 Mg3 La3 66.07(17) 2_554 . ?
Mg2 Mg3 La3 169.6(5) 9_556 . ?
Mg1 Mg3 La3 113.83(15) 5_445 . ?
Mg1 Mg3 La3 113.83(15) 7_545 . ?
La2 Mg3 La3 67.2(2) . . ?
La2 Mg3 La3 67.2(2) 3 . ?
La3 Mg3 La3 124.3(4) 10_556 . ?
Mg2 Mg3 La8 65.10(11) 2_554 12 ?
Mg2 Mg3 La8 111.8(2) 9_556 12 ?
Mg1 Mg3 La8 62.14(17) 5_445 12 ?
Mg1 Mg3 La8 113.5(4) 7_545 12 ?
La2 Mg3 La8 120.8(3) . 12 ?
La2 Mg3 La8 63.49(11) 3 12 ?
La3 Mg3 La8 117.70(17) 10_556 12 ?
La3 Mg3 La8 64.68(7) . 12 ?
Mg2 Mg3 La8 111.8(2) 2_554 10_556 ?
Mg2 Mg3 La8 65.10(11) 9_556 10_556 ?
Mg1 Mg3 La8 113.5(4) 5_445 10_556 ?
Mg1 Mg3 La8 62.14(17) 7_545 10_556 ?
La2 Mg3 La8 63.49(11) . 10_556 ?
La2 Mg3 La8 120.8(3) 3 10_556 ?
La3 Mg3 La8 64.68(7) 10_556 10_556 ?
La3 Mg3 La8 117.70(17) . 10_556 ?
La8 Mg3 La8 175.4(5) 12 10_556 ?
Mg2 Mg3 La8 65.10(11) 2_554 . ?
Mg2 Mg3 La8 111.8(2) 9_556 . ?
Mg1 Mg3 La8 113.5(4) 5_445 . ?
Mg1 Mg3 La8 62.14(17) 7_545 . ?
La2 Mg3 La8 63.49(11) . . ?
La2 Mg3 La8 120.8(3) 3 . ?
La3 Mg3 La8 117.70(17) 10_556 . ?
La3 Mg3 La8 64.68(7) . . ?
La8 Mg3 La8 119.17(4) 12 . ?
La8 Mg3 La8 60.62(3) 10_556 . ?
Mg2 Mg3 La8 111.8(2) 2_554 3 ?
Mg2 Mg3 La8 65.10(11) 9_556 3 ?
Mg1 Mg3 La8 62.14(17) 5_445 3 ?
Mg1 Mg3 La8 113.5(4) 7_545 3 ?
La2 Mg3 La8 120.8(3) . 3 ?
La2 Mg3 La8 63.49(11) 3 3 ?
La3 Mg3 La8 64.68(7) 10_556 3 ?
La3 Mg3 La8 117.70(17) . 3 ?
La8 Mg3 La8 60.62(3) 12 3 ?
La8 Mg3 La8 119.17(4) 10_556 3 ?
La8 Mg3 La8 175.4(5) . 3 ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
La1 Mg1 3.409(10) . ?
La1 Mg1 3.409(10) 3 ?
La1 La8 3.7054(16) 7 ?
La1 La8 3.7054(16) 16 ?
La1 La8 3.7054(16) 14_456 ?
La1 La8 3.7054(16) 5_455 ?
La1 La2 3.780(2) 3 ?
La1 La2 3.780(2) . ?
La1 La4 3.8864(11) 12 ?
La1 La4 3.8864(11) . ?
La1 La4 3.8864(11) 10_556 ?
La1 La4 3.8864(11) 3 ?
La2 Mg1 3.400(10) . ?
La2 Mg3 3.410(13) . ?
La2 La8 3.7094(15) . ?
La2 La8 3.7094(15) 10_556 ?
La2 La5 3.7112(14) 14_546 ?
La2 La5 3.7112(14) 5_545 ?
La2 La2 3.792(3) 3 ?
La2 La4 3.8852(12) 10_556 ?
La2 La4 3.8852(12) . ?
La2 La3 3.8915(14) . ?
La2 La3 3.8915(14) 10_556 ?
La3 Ni3 2.933(2) 12 ?
La3 Ni3 2.933(2) . ?
La3 Ni1 3.617(3) . ?
La3 Mg3 3.619(7) . ?
La3 Mg2 3.715(8) 2_554 ?
La3 La9 3.7805(15) 5_445 ?
La3 La9 3.7805(15) 16_545 ?
La3 La7 3.8117(15) 12 ?
La3 La7 3.8117(15) . ?
La3 La4 3.8521(15) . ?
La3 La4 3.8521(15) 12 ?
La3 La8 3.8786(12) 12 ?
La4 Ni2 2.924(2) . ?
La4 Ni3 2.929(2) . ?
La4 Mg1 3.633(5) . ?
La4 Mg2 3.730(5) 6_554 ?
La4 La9 3.7438(13) . ?
La4 La6 3.7876(12) 6_554 ?
La4 La7 3.8033(13) . ?
La4 La4 3.8369(19) 12 ?
La4 La12 3.8623(15) . ?
La4 La8 3.8779(13) 16 ?
La5 Ni3 2.920(2) 5_455 ?
La5 Ni3 2.920(2) 16 ?
La5 Ni5 2.922(4) . ?
La5 La6 3.6289(19) 2_564 ?
La5 Mg1 3.630(7) 7 ?
La5 Mg1 3.630(7) 5_455 ?
La5 Mg2 3.656(8) 2_564 ?
La5 La5 3.671(3) 10_556 ?
La5 La2 3.7112(14) 7 ?
La5 La2 3.7112(14) 5_455 ?
La5 La14 3.8490(19) . ?
La5 La4 3.8907(12) 16 ?
La6 Ni4 2.871(2) 15_456 ?
La6 Ni4 2.871(2) 6 ?
La6 Mg2 3.559(10) . ?
La6 La14 3.6018(19) 2_565 ?
La6 La5 3.6289(19) 2_565 ?
La6 La15 3.630(2) . ?
La6 La13 3.7493(19) . ?
La6 La7 3.7499(12) 6 ?
La6 La7 3.7499(12) 15_456 ?
La6 La4 3.7876(12) 6 ?
La6 La4 3.7876(12) 15_456 ?
La6 La9 3.9391(15) 15_456 ?
La7 Ni4 2.953(2) . ?
La7 Ni1 2.958(3) . ?
La7 Ni3 3.010(2) . ?
La7 La6 3.7499(12) 6_554 ?
La7 La9 3.7740(14) 16_545 ?
La7 La11 3.7971(14) . ?
La7 La14 3.8463(12) 5_545 ?
La7 La15 3.8690(13) 6_554 ?
La7 La12 3.8723(15) . ?
La7 La10 3.8995(13) . ?
La8 Ni5 2.910(2) 5_545 ?
La8 Ni3 2.916(2) . ?
La8 Ni2 2.938(3) 5_545 ?
La8 La9 3.6178(13) 16_545 ?
La8 Mg1 3.622(7) 7_545 ?
La8 Mg3 3.6310(11) . ?
La8 La8 3.6648(18) 10_556 ?
La8 Mg2 3.675(5) 2_554 ?
La8 La1 3.7054(16) 5_545 ?
La8 La14 3.8455(15) 5_545 ?
La8 La4 3.8779(13) 16_545 ?
La9 Ni1 2.856(2) 5 ?
La9 Ni4 2.858(2) . ?
La9 Mg2 3.546(9) 6_554 ?
La9 La14 3.6048(12) . ?
La9 La8 3.6178(13) 16 ?
La9 La16 3.7215(14) 16 ?
La9 La13 3.7693(15) 6_554 ?
La9 La7 3.7740(14) 16 ?
La9 La3 3.7805(15) 5 ?
La9 La12 3.8063(12) . ?
La9 La6 3.9391(15) 6_554 ?
La10 Ni6 2.769(2) . ?
La10 Ni4 2.907(2) . ?
La10 La16 3.6951(13) 16 ?
La10 La10 3.7412(18) 13 ?
La10 La15 3.7756(13) 6_554 ?
La10 La15 3.7909(16) 10_556 ?
La10 La13 3.7944(12) 6_554 ?
La10 La12 3.8129(15) . ?
La10 La16 3.8318(13) 13 ?
La10 La11 3.9058(12) 13 ?
La10 La11 3.9173(15) . ?
La11 Ni1 2.880(3) . ?
La11 Ni7 3.0229(19) 9 ?
La11 Ni7 3.0229(19) . ?
La11 La16 3.7760(12) 12 ?
La11 La16 3.7760(12) . ?
La11 La13 3.7769(18) 10_556 ?
La11 La7 3.7971(14) 12 ?
La11 La13 3.8104(19) 2_554 ?
La11 La10 3.9058(12) 8_455 ?
La11 La10 3.9058(12) 13 ?
La12 Ni4 2.933(2) 12 ?
La12 Ni4 2.933(2) . ?
La12 Ni2 3.101(3) . ?
La12 La9 3.8063(12) 12 ?
La12 La10 3.8129(15) 12 ?
La12 La4 3.8623(15) 12 ?
La12 La7 3.8723(15) 12 ?
La12 La16 3.8764(15) 16 ?
La13 Ni7 2.9378(19) 2 ?
La13 Ni7 2.9378(19) 10_556 ?
La13 Ni4 2.968(2) 6 ?
La13 Ni4 2.968(2) 15_456 ?
La13 Ni1 2.995(3) 2 ?
La13 La16 3.7276(12) 2 ?
La13 La16 3.7276(12) 11_556 ?
La13 La15 3.764(2) . ?
La13 La9 3.7693(14) 6 ?
La13 La9 3.7693(15) 15_456 ?
La13 La11 3.7769(18) 10_556 ?
La14 Ni2 2.948(3) . ?
La14 Ni3 2.980(2) 16 ?
La14 Ni3 2.980(2) 5_455 ?
La14 La6 3.6018(19) 2_564 ?
La14 La9 3.6048(12) 12 ?
La14 La8 3.8455(15) 16 ?
La14 La8 3.8455(15) 5_455 ?
La14 La7 3.8463(12) 16 ?
La14 La7 3.8463(12) 5_455 ?
La15 Ni6 3.571(4) 10_556 ?
La15 La16 3.7450(17) 6 ?
La15 La16 3.7450(17) 15_456 ?
La15 La10 3.7756(13) 15_456 ?
La15 La10 3.7756(13) 6 ?
La15 La10 3.7909(16) 3 ?
La15 La10 3.7909(16) 10_556 ?
La15 La7 3.8690(13) 6 ?
La15 La7 3.8690(13) 15_456 ?
La15 La11 4.080(2) 10_556 ?
La16 Ni7 2.782(3) . ?
La16 Ni6 3.013(3) 13 ?
La16 Ni6 3.018(3) 5_545 ?
La16 La10 3.6951(13) 16_545 ?
La16 La9 3.7215(14) 16_545 ?
La16 La13 3.7276(12) 2_554 ?
La16 La16 3.7301(19) 12_655 ?
La16 La15 3.7450(17) 6_554 ?
La16 La10 3.8318(13) 13 ?
La16 La12 3.8764(15) 5_545 ?
Ni1 La9 2.856(2) 16_545 ?
Ni1 La9 2.856(2) 5_445 ?
Ni1 La7 2.958(2) 12 ?
Ni1 La13 2.995(3) 2_554 ?
Ni2 La4 2.924(2) 12 ?
Ni2 La8 2.938(3) 16 ?
Ni2 La8 2.938(3) 5_455 ?
Ni3 La5 2.920(2) 5_545 ?
Ni3 La14 2.980(2) 5_545 ?
Ni4 La6 2.871(2) 6_554 ?
Ni4 La13 2.968(2) 6_554 ?
Ni5 La8 2.910(2) 5_455 ?
Ni5 La8 2.910(2) 7 ?
Ni5 La8 2.910(2) 16 ?
Ni5 La8 2.910(2) 14_456 ?
Ni5 La5 2.922(4) 10_556 ?
Ni6 Ni6 2.532(6) 9_565 ?
Ni6 La10 2.769(2) 12 ?
Ni6 La16 3.013(3) 8_455 ?
Ni6 La16 3.013(3) 13 ?
Ni6 La16 3.018(3) 16 ?
Ni6 La16 3.018(3) 5_455 ?
Ni6 La15 3.571(4) 10_556 ?
Ni7 Ni7 2.599(7) 9 ?
Ni7 La16 2.782(3) 4 ?
Ni7 La13 2.9378(19) 10_556 ?
Ni7 La13 2.9378(19) 2_554 ?
Ni7 La11 3.0229(19) 9 ?
Mg1 Mg2 3.155(11) 13_556 ?
Mg1 Mg2 3.155(11) 6_554 ?
Mg1 Mg3 3.374(16) 5 ?
Mg1 Mg1 3.39(2) 3_655 ?
Mg1 La8 3.622(7) 7 ?
Mg1 La8 3.622(7) 16 ?
Mg1 La5 3.630(7) 5_545 ?
Mg1 La5 3.630(7) 14_546 ?
Mg1 La4 3.633(5) 10_556 ?
Mg2 Mg1 3.155(11) 13_556 ?
Mg2 Mg1 3.155(11) 15_456 ?
Mg2 Mg3 3.159(14) 9_556 ?
Mg2 La9 3.546(9) 15_456 ?
Mg2 La9 3.546(9) 6 ?
Mg2 La5 3.656(8) 2_565 ?
Mg2 La8 3.675(5) 2 ?
Mg2 La8 3.675(5) 11_556 ?
Mg2 La3 3.715(8) 2 ?
Mg2 La4 3.730(5) 6 ?
Mg2 La4 3.730(5) 15_456 ?
Mg3 Mg2 3.159(14) 2_554 ?
Mg3 Mg2 3.159(14) 9_556 ?
Mg3 Mg1 3.374(16) 5_445 ?
Mg3 Mg1 3.374(16) 7_545 ?
Mg3 La2 3.410(12) 3 ?
Mg3 La3 3.619(7) 10_556 ?
Mg3 La8 3.6310(11) 12 ?
Mg3 La8 3.6310(11) 10_556 ?
Mg3 La8 3.6310(11) 3 ?
